Graphene

Graphene (/ˈɡræfiːn/)[1] is a variety of the element carbon which occurs naturally in small amounts. In graphene, the carbon forms a sheet of interlocked atoms as hexagons one carbon atom thick. The result resembles the face of a honeycomb. When many hundreds of graphene layers build up, they are called graphite.

Commonly known types of carbon are diamond and graphite. In 1947, the Canadian physicist P. R. Wallace suggested carbon could also exist in sheets. The German chemist Hanns-Peter Boehm and coworkers isolated single sheets from graphite, giving them the name graphene in 1986. In 2004, the material was characterized by Andre Geim and Konstantin Novoselov at the University of Manchester, England. They received the 2010 Nobel Prize in Physics for their experiments.

In technical terms, graphene is a carbon allotrope consisting of a single layer of atoms arranged in a honeycomb planar nanostructure.[2][3] The name "graphene" is derived from "graphite" and the suffix -ene, indicating the presence of double bonds within the carbon structure.

Graphene is known for its exceptionally high tensile strength, electrical conductivity, transparency, and being the thinnest two-dimensional material in the world.[4] Despite the nearly transparent nature of a single graphene sheet, graphite (formed from stacked layers of graphene) appears black because it absorbs all visible light wavelengths.[5][6] On a microscopic scale, graphene is the strongest material ever measured.[7][8]

Photograph of a suspended graphene membrane in transmitted light. This one-atom-thick material can be seen with the naked eye because it absorbs approximately 2.3% of light.[5][6]

The existence of graphene was first theorized in 1947 by Philip R. Wallace during his research on graphite's electronic properties, while the term graphene was first defined by Hanns-Peter Boehm in 1987.[9] In 2004, the material was isolated and characterized by Andre Geim and Konstantin Novoselov at the University of Manchester[10][11] using a piece of graphite and adhesive tape.[12] In 2010, Geim and Novoselov were awarded the Nobel Prize in Physics for their "groundbreaking experiments regarding the two-dimensional material graphene".[13] While small amounts of graphene are easy to produce using the method by which it was originally isolated, attempts to scale and automate the manufacturing process for mass production have had limited success out of concern for cost-effectiveness and quality control.[14][15] The global graphene market was $9 million in 2012,[16] with most of the demand from research and development in semiconductors, electronics, electric batteries,[17] and composites.

The IUPAC (International Union of Pure and Applied Chemistry) advises using the term "graphite" for the three-dimensional material and reserving "graphene" for discussions about the properties or reactions of single-atom layers.[18] A narrower definition, of "isolated or free-standing graphene", requires that the layer be sufficiently isolated from its environment,[19] but would include layers suspended or transferred to silicon dioxide or silicon carbide.[20]

## Contents

* 1 History
* 1.1 Structure of graphite and its intercalation compounds
* 1.2 Observations of thin graphite layers and related structures
* 1.3 Full isolation and characterization
* 1.4 Exploring commercial applications
* 2 Structure
* 2.1 Bonding
* 2.2 Geometry
* 2.3 Stability
* 3 Electronic properties
* 3.1 Electronic spectrum
* 3.2 Dispersion relation
* 3.3 Single-atom wave propagation
* 3.4 Ambipolar electron and hole transport
* 3.4.1 Electrical conductivity and charge transport
* 3.5 Chiral half-integer quantum Hall effect
* 3.5.1 Quantum hall effect in graphene
* 3.5.2 Chiral electrons and anomalies
* 3.5.3 Experimental observations
* 3.6 "Massive" electrons
* 3.7 Inertial effect and kinetic inductance
* 4 Interactions and phenomena
* 4.1 Strong magnetic fields
* 4.2 Casimir effect
* 4.3 Van der Waals force
* 4.4 Permittivity
* 5 Optical properties
* 5.1 Multi-parametric surface plasmon resonance
* 5.2 Tunable band gap and optical response
* 5.3 Graphene-based Bragg grating
* 5.4 Saturable absorption
* 5.5 Nonlinear Kerr effect
* 6 Excitonic properties
* 6.1 Spin transport
* 7 Magnetic properties
* 7.1 Strong magnetic fields
* 7.2 Spintronic properties
* 7.3 Magnetic substrates
* 8 Mechanical properties
* 8.1 Fracture toughness
* 8.2 Polycrystalline graphene
* 9 Other properties
* 9.1 Thermal conductivity
* 9.2 Chemical properties
* 9.3 Biological properties
* 9.4 Support substrate
* 10 Graphene layers and structural variants
* 10.1 Monolayer sheets
* 10.2 Bilayer graphene
* 10.3 Turbostratic
* 10.4 Graphene superlattices
* 11 Nanostructured graphene forms
* 11.1 Graphene nanoribbons
* 11.2 Graphene quantum dots
* 12 Modified and functionalized graphene
* 12.1 Graphene oxide
* 12.2 Chemical modification
* 12.3 Graphene ligand/complex
* 13 Advanced graphene structures
* 13.1 Graphene fiber
* 13.2 3D graphene
* 13.3 Pillared graphene
* 13.4 Reinforced graphene
* 13.5 Molded graphene
* 14 Specialized graphene configurations
* 14.1 Graphene aerogel
* 14.2 Graphene nanocoil
* 14.3 Crumpled graphene
* 15 Mechanical synthesis
* 15.1 Bottom-up and top-down methods
* 15.2 Micro-mechanical cleavage
* 15.3 Exfoliation techniques
* 15.3.1 Mechanical exfoliation
* 15.3.2 Liquid phase exfoliation
* 15.3.3 Exfoliation with supercritical carbon dioxide
* 15.4 Splitting monolayer carbon allotropes
* 16 Chemical synthesis
* 16.1 Graphite oxide reduction
* 16.2 Molten salts
* 16.3 Electrochemical synthesis
* 16.4 Hydrothermal self-assembly
* 16.5 Sodium ethoxide pyrolysis
* 16.6 Microwave-assisted oxidation
* 16.7 Thermal decomposition of silicon carbide
* 17 Vapor deposition and growth techniques
* 17.1 Chemical vapor deposition
* 17.1.1 Epitaxy
* 17.1.2 Metal substrates
* 17.1.3 Roll-to-roll
* 17.1.4 Cold wall
* 17.1.5 Wafer scale CVD graphene
* 17.2 Solvent interface trapping method (SITM)
* 17.3 Carbon dioxide reduction
* 17.4 Supersonic spray
* 17.5 Laser
* 17.6 Flash Joule heating
* 17.7 Ion implantation
* 17.8 CMOS-compatible graphene
* 18 Simulation
* 19 Graphene analogs
* 20 Applications
* 21 Toxicity
* 22 See also
* 23 References
* 24 External links

## History

Main article: Chemistry:Discovery of graphene

A lump of graphite, a graphene transistor, and a tape dispenser signed by Andre Geim. Donated to the Nobel Museum in Stockholm by Geim and Konstantin Novoselov in 2010.

### Structure of graphite and its intercalation compounds

In 1859, Benjamin Brodie noted the highly lamellar structure of thermally reduced graphite oxide.[21][22] Researchers used X-ray crystallography in an attempt to determine the structure of graphite. The lack of large single crystal graphite specimens contributed to the independent development of X-ray powder diffraction by Peter Debye and Paul Scherrer in 1915, and Albert Hull in 1916.[23][24][25] However, neither of their proposed structures was correct. In 1918, Volkmar Kohlschütter and P. Haenni described the properties of graphite oxide paper.[26] The structure of graphite was successfully determined from single-crystal X-ray diffraction by J. D. Bernal in 1924,[27] while subsequent research tweaked the unit cell parameters.[28][29]

The theory of graphene was first explored by P. R. Wallace in 1947 as a starting point for understanding the electronic properties of 3D graphite. The emergent massless Dirac equation was separately pointed out in 1984 by Gordon Walter Semenoff,[30] and by David P. Vincenzo and Eugene J. Mele.[31] Semenoff emphasized the occurrence in a magnetic field of an electronic Landau level precisely at the Dirac point. This level is responsible for the anomalous integer Quantum Hall effect.[32][33][34]

### Observations of thin graphite layers and related structures

Transmission electron microscopy (TEM) images of thin graphite samples consisting of a few graphene layers were published by G. Ruess and F. Vogt in 1948.[35] Eventually, single layers were also observed directly.[36] Single layers of graphite were also observed by transmission electron microscopy within bulk materials, particularly inside soot obtained by chemical exfoliation.[37]

From 1961 to 1962, Hanns-Peter Boehm published a study of extremely thin flakes of graphite.[38] The study measured flakes as small as ~0.4 nm, which is around 3 atomic layers of amorphous carbon. This was the best possible resolution for TEMs in the 1960s. However, it is impossible to distinguish between suspended monolayer and multilayer graphene by their TEM contrasts, and the only known method is to analyze the relative intensities of various diffraction spots.[36] The first reliable TEM observations of monolayers are likely given in references 24 and 26 of Geim and Novoselov's 2007 review.[2]

In 1975, van Bommel et al. epitaxially grew a single layer of graphite on top of silicon carbide.[39] Others grew single layers of carbon atoms on other materials.[40][41] This "epitaxial graphene" consists of a single-atom-thick hexagonal lattice of sp2-bonded carbon atoms, as in free-standing graphene. However, there is significant charge transfer between the two materials and, in some cases, hybridization between the d-orbitals of the substrate atoms and π orbitals of graphene, which significantly alter the electronic structure compared to that of free-standing graphene.

Boehm et al. coined the term "graphene" for the hypothetical single-layer structure in 1986.[42] The term was used again in 1987 to describe single sheets of graphite as a constituent of graphite intercalation compounds,[43] which can be seen as crystalline salts of the intercalant and graphene. It was also used in the descriptions of carbon nanotubes by R. Saito and Mildred and Gene Dresselhaus in 1992,[44] and in the description of polycyclic aromatic hydrocarbons in 2000 by S. Wang and others.[45]

Efforts to make thin films of graphite by mechanical exfoliation started in 1990.[46] Initial attempts employed exfoliation techniques similar to the drawing method. Multilayer samples down to 10 nm in thickness were obtained.[2]

In 2002, Robert B. Rutherford and Richard L. Dudman filed for a patent in the US on a method to produce graphene by repeatedly peeling off layers from a graphite flake adhered to a substrate, achieving a graphite thickness of 0.00001 inches (0.00025 millimetres). The key to success was the ability to quickly and efficiently identify graphene flakes on the substrate using optical microscopy, which provided a small but visible contrast between the graphene and the substrate.[47]

Another U.S. patent was filed in the same year by Bor Z. Jang and Wen C. Huang for a method to produce graphene-based on exfoliation followed by attrition.[48]

In 2014, inventor Larry Fullerton patented a process for producing single-layer graphene sheets by graphene's strong diamagnetic properties.[49]

### Full isolation and characterization

Andre Geim and Konstantin Novoselov at the Nobel Laureate press conference, Royal Swedish Academy of Sciences, 2010.

Graphene was properly isolated and characterized in 2004 by Andre Geim and Konstantin Novoselov at the University of Manchester.[10][11] They pulled graphene layers from graphite with a common adhesive tape in a process called micro-mechanical cleavage, colloquially referred to as the Scotch tape technique.[50] The graphene flakes were then transferred onto a thin silicon dioxide layer on a silicon plate ("wafer"). The silica electrically isolated the graphene and weakly interacted with it, providing nearly charge-neutral graphene layers. The silicon beneath the SiO2 could be used as a "back gate" electrode to vary the charge density in the graphene over a wide range.

This work resulted in the two winning the Nobel Prize in Physics in 2010 for their groundbreaking experiments with graphene.[50][51][52] Their publication and the surprisingly easy preparation method that they described, sparked a "graphene gold rush". Research expanded and split off into many different subfields, exploring different exceptional properties of the material—quantum mechanical, electrical, chemical, mechanical, optical, magnetic, etc.

### Exploring commercial applications

Since the early 2000s, several companies and research laboratories have been working to develop commercial applications of graphene. In 2014, a National Graphene Institute was established with that purpose at the University of Manchester, with a £60 million initial funding.[53] In North East England two commercial manufacturers, Applied Graphene Materials[54] and Thomas Swan Limited[55][56] have begun manufacturing. Cambridge Nanosystems[57] is a large-scale graphene powder production facility in East Anglia.

## Structure

Graphene is a single layer of carbon atoms tightly bound in a hexagonal honeycomb lattice. It is an allotrope of carbon in the form of a plane of sp2-bonded atoms with a molecular bond length R = 0.142 nm (1.42 Å).

The area of a hexagon of side R being 332R2, one hexagonal unit of graphene has an area of 3320.1422=0.0524 nm2. There are two carbon atoms per unit, together having a mass of 212N0=.0399×10−18 mg. The (two-dimensional) density of graphene is therefore 0.0399/0.0542=0.762 mg per square meter. A kilogram of graphene therefore has an area of 106/0.762=1.312×106 m2 or 131.2 hectares.

In a graphene sheet, each atom is connected to its three nearest carbon neighbors by σ-bonds, and a delocalized π-bond, which contributes to a valence band that extends over the whole sheet. This type of bonding is also seen in polycyclic aromatic hydrocarbons.[58][37] The valence band is touched by a conduction band, making graphene a semimetal with unusual electronic properties that are best described by theories for massless relativistic particles.[2] Charge carriers in graphene show linear, rather than quadratic, dependence of energy on momentum, and field-effect transistors with graphene can be made that show bipolar conduction. Charge transport is ballistic over long distances; the material exhibits large quantum oscillations and large nonlinear diamagnetism.[59]

### Bonding

Carbon orbitals 2s, 2px, 2py form the hybrid orbital sp2 with three major lobes at 120°. The remaining orbital, pz, extends out of the graphene's plane. Sigma and pi bonds in graphene. Sigma bonds result from an overlap of sp2 hybrid orbitals, whereas pi bonds emerge from tunneling between the protruding pz orbitals.

Three of the four outer-shell electrons of each atom in a graphene sheet occupy three sp2 hybrid orbitals – a combination of orbitals s, px and py — that are shared with the three nearest atoms, forming σ-bonds. The length of these bonds is about 0.142 nanometers.[60][61]

The remaining outer-shell electron occupies a pz orbital that is oriented perpendicularly to the plane. These orbitals hybridize together to form two half-filled bands of free-moving electrons, π, and π∗, which are responsible for most of graphene's notable electronic properties.[60] Recent quantitative estimates of aromatic stabilization and limiting size derived from the enthalpies of hydrogenation (ΔHhydro) agree well with the literature reports.[62]

Graphene sheets stack to form graphite with an interplanar spacing of 0.335 nm (3.35 Å).[63]

Graphene sheets in solid form usually show evidence in diffraction for graphite's (002) layering. This is true of some single-walled nanostructures.[64] However, unlayered graphene displaying only (hk0) rings have been observed in the core of presolar graphite onions.[65] TEM studies show faceting at defects in flat graphene sheets[66] and suggest a role for two-dimensional crystallization from a melt.

### Geometry

Scanning probe microscopy image of graphene

The hexagonal lattice structure of isolated, single-layer graphene can be directly seen with transmission electron microscopy (TEM) of sheets of graphene suspended between bars of a metallic grid.[36] Some of these images showed a "rippling" of the flat sheet, with an amplitude of about one nanometer. These ripples may be intrinsic to the material as a result of the instability of two-dimensional crystals,[2][67][68] or may originate from the ubiquitous dirt seen in all TEM images of graphene. Photoresist residue, which must be removed to obtain atomic-resolution images, may be the "adsorbates" observed in TEM images, and may explain the observed rippling.[69]

The hexagonal structure is also seen in scanning tunneling microscope (STM) images of graphene supported on silicon dioxide substrates[70] The rippling seen in these images is caused by the conformation of graphene to the substrates' lattice and is not intrinsic.[70]

### Stability

Ab initio calculations show that a graphene sheet is thermodynamically unstable if its size is less than about 20 nm and becomes the most stable fullerene (as within graphite) only for molecules larger than 24,000 atoms.[71]

## Electronic properties

Main article: Physics:Electronic properties of graphene

Electronic band structure of graphene. Valence and conduction bands meet at the six vertices of the hexagonal Brillouin zone and form linearly dispersing Dirac cones.

Graphene is a zero-gap semiconductor because its conduction and valence bands meet at the Dirac points. The Dirac points are six locations in momentum space on the edge of the Brillouin zone, divided into two non-equivalent sets of three points. These sets are labeled K and K'. These sets give graphene a valley degeneracy of gv=2. In contrast, for traditional semiconductors, the primary point of interest is generally Γ, where momentum is zero.[60]

If the in-plane direction is confined rather than infinite, its electronic structure changes. These confined structures are referred to as graphene nanoribbons. If the nanoribbon has a "zig-zag" edge, the bandgap remains zero. If it has an "armchair" edge, the bandgap is non-zero.

Graphene's honeycomb structure can be viewed as two interleaving triangular lattices. This perspective has been used to calculate the band structure for a single graphite layer using a tight-binding approximation.[60]

### Electronic spectrum

Electrons propagating through the graphene honeycomb lattice effectively lose their mass, producing quasi-particles described by a 2D analogue of the Dirac equation rather than the Schrödinger equation for spin-⁠1/2⁠ particles.[72][73]

### Dispersion relation

File:Graphene and Dirac Cones.ogvElectronic band structure and Dirac cones, with effect of doping

The cleavage technique led directly to the first observation of the anomalous quantum Hall effect in graphene in 2005 by Geim's group and by Philip Kim and Yuanbo Zhang. This effect provided direct evidence of graphene's theoretically predicted Berry's phase of massless Dirac fermions and proof of the Dirac fermion nature of electrons.[32][34] These effects were previously observed in bulk graphite by Yakov Kopelevich, Igor A. Luk'yanchuk, and others, in 2003–2004.[74][75]

When atoms are placed onto the graphene hexagonal lattice, the overlap between the pz(π) orbitals and the s or the px and py orbitals is zero by symmetry. Therefore, pz electrons forming the π bands in graphene can be treated independently. Within this π-band approximation, using a conventional tight-binding model, the dispersion relation (restricted to first-nearest-neighbor interactions only) that produces the energy of the electrons with wave vector k is:[30][76]

E(kx,ky)=±γ01+4cos212akx+4cos⁡12akx⋅cos⁡32aky

with the nearest-neighbor (π orbitals) hopping energy γ0 ≈ 2.8 eV and the lattice constant a ≈ 2.46 Å. The conduction and valence bands correspond to the different signs. With one pz electron per atom in this model, the valence band is fully occupied, while the conduction band is vacant. The two bands touch at the zone corners (the K point in the Brillouin zone), where there is a zero density of states but no band gap. Thus, graphene exhibits a semi-metallic (or zero-gap semiconductor) character, although this is not true for a graphene sheet rolled into a carbon nanotube due to its curvature. Two of the six Dirac points are independent, while the rest are equivalent by symmetry. Near the K-points, the energy depends linearly on the wave vector, similar to a relativistic particle.[30][77] Since an elementary cell of the lattice has a basis of two atoms, the wave function has an effective 2-spinor structure.

Consequently, at low energies even neglecting the true spin, electrons can be described by an equation formally equivalent to the massless Dirac equation. Hence, the electrons and holes are called Dirac fermions.[30] This pseudo-relativistic description is restricted to the chiral limit, i.e., to vanishing rest mass M0, leading to interesting additional features:[30][78]

vFσ→⋅∇ψ(𝐫)=Eψ(𝐫).

Here vF ~ 106 m/s (.003 c) is the Fermi velocity in graphene, which replaces the velocity of light in the Dirac theory; σ→ is the vector of the Pauli matrices, ψ(𝐫) is the two-component wave function of the electrons, and E is their energy.[72]

The equation describing the electrons' linear dispersion relation is:

E(q)=ℏvFq

where the wavevector q is measured from the Brillouin zone vertex K, q=|𝐤−K|, and the zero of energy is set to coincide with the Dirac point. The equation uses a pseudospin matrix formula that describes two sublattices of the honeycomb lattice.[77]

### Single-atom wave propagation

Electron waves in graphene propagate within a single-atom layer, making them sensitive to the proximity of other materials such as high-κ dielectrics, superconductors, and ferromagnets.

### Ambipolar electron and hole transport

When the gate voltage in a field effect graphene device is changed from positive to negative, conduction switches from electrons to holes. The charge carrier concentration is proportional to the applied voltage. Graphene is neutral at zero gate voltage and resistivity is at its maximum because of the dearth of charge carriers. The rapid fall of resistivity when carriers are injected shows their high mobility, here of the order of 5000 cm2/Vs. n-Si/SiO2 substrate, T=1K.[2]

Graphene exhibits high electron mobility at room temperature, with values reported in excess of 15000 cm2⋅V−1⋅s−1.[2] Hole and electron mobilities are nearly identical.[73] The mobility is independent of temperature between 10 K and 100 K,[32][79][80] showing minimal change even at room temperature (300 K),[2] suggesting that the dominant scattering mechanism is defect scattering. Scattering by graphene's acoustic phonons intrinsically limits room temperature mobility in freestanding graphene to 200000 cm2⋅V−1⋅s−1 at a carrier density of 1012 cm−2.[80][81]

The corresponding resistivity of graphene sheets is 10−8 Ω⋅m, lower than the resistivity of silver, which is the lowest known at room temperature.[82] However, on SiO2 substrates, electron scattering by optical phonons of the substrate has a more significant effect than scattering by graphene's phonons, limiting mobility to 40000 cm2⋅V−1⋅s−1.[80]

Charge transport can be affected by the adsorption of contaminants such as water and oxygen molecules, leading to non-repetitive and large hysteresis I-V characteristics. Researchers need to conduct electrical measurements in a vacuum. Coating the graphene surface with materials such as SiN, PMMA or h-BN has been proposed for protection. In January 2015, the first stable graphene device operation in the air over several weeks was reported for graphene whose surface was protected by aluminum oxide.[83][84] In 2015, lithium-coated graphene exhibited superconductivity, a first for graphene.[85]

Electrical resistance in 40-nanometer-wide nanoribbons of epitaxial graphene changes in discrete steps. The ribbons' conductance exceeds predictions by a factor of 10. The ribbons can function more like optical waveguides or quantum dots, allowing electrons to flow smoothly along the ribbon edges. In copper, resistance increases proportionally with length as electrons encounter impurities.[86][87]

Transport is dominated by two modes: one ballistic and temperature-independent, and the other thermally activated. Ballistic electrons resemble those in cylindrical carbon nanotubes. At room temperature, resistance increases abruptly at a specific length—the ballistic mode at 16 micrometers and the thermally activated mode at 160 nanometers (1% of the former length).[86]

Graphene electrons can traverse micrometer distances without scattering, even at room temperature.[72]

#### Electrical conductivity and charge transport

Despite zero carrier density near the Dirac points, graphene exhibits a minimum conductivity on the order of 4e2/h. The origin of this minimum conductivity is still unclear. However, rippling of the graphene sheet or ionized impurities in the SiO2 substrate may lead to local puddles of carriers that allow conduction.[73] Several theories suggest that the minimum conductivity should be 4e2/(πh); however, most measurements are of the order of 4e2/h or greater[2] and depend on impurity concentration.[88]

Near zero carrier density, graphene exhibits positive photoconductivity and negative photoconductivity at high carrier density, governed by the interplay between photoinduced changes of both the Drude weight and the carrier scattering rate.[89]

Graphene doped with various gaseous species (both acceptors and donors) can be returned to an undoped state by gentle heating in a vacuum.[88][90] Even for dopant concentrations in excess of 1012 cm−2, carrier mobility exhibits no observable change.[90] Graphene doped with potassium in ultra-high vacuum at low temperature can reduce mobility 20-fold.[88][91] The mobility reduction is reversible on heating the graphene to remove the potassium.

Due to graphene's two dimensions, charge fractionalization (where the apparent charge of individual pseudoparticles in low-dimensional systems is less than a single quantum)[92] is thought to occur. It may therefore be a suitable material for constructing quantum computers[93] using anyonic circuits.[94]

### Chiral half-integer quantum Hall effect

Landau levels in graphene appear at energies proportional to √N, in contrast to the standard sequence that goes as N \+ ⁠1/2⁠.[2]

#### Quantum hall effect in graphene

The quantum Hall effect is a quantum mechanical version of the Hall effect, which is the production of transverse (perpendicular to the main current) conductivity in the presence of a magnetic field. The quantization of the Hall effect σxy at integer multiples (the "Landau level") of the basic quantity e2/h (where e is the elementary electric charge and h is the Planck constant). It can usually be observed only in very clean silicon or gallium arsenide solids at temperatures around 3 K and very high magnetic fields.

Graphene shows the quantum Hall effect: the conductivity quantization is unusual in that the sequence of steps is shifted by 1/2 with respect to the standard sequence and with an additional factor of 4. Graphene's Hall conductivity is σxy=±4⋅(N+1/2)e2/h, where N is the Landau level and the double valley and double spin degeneracies give the factor of 4.[2] These anomalies are present not only at extremely low temperatures but also at room temperature, i.e. at roughly 20 °C (293 K).[32]

#### Chiral electrons and anomalies

This behavior is a direct result of graphene's chiral, massless Dirac electrons.[2][95] In a magnetic field, their spectrum has a Landau level with energy precisely at the Dirac point. This level is a consequence of the Atiyah–Singer index theorem and is half-filled in neutral graphene,[30] leading to the "+1/2" in the Hall conductivity.[33] Bilayer graphene also shows the quantum Hall effect, but with only one of the two anomalies (i.e. σxy=±4⋅N⋅e2/h). In the second anomaly, the first plateau at N = 0 is absent, indicating that bilayer graphene stays metallic at the neutrality point.[2]

Chiral half-integer quantum Hall effect in graphene. Plateaux in transverse conductivity appear at half-integer multiples of 4e2/h.[2]

Unlike normal metals, graphene's longitudinal resistance shows maxima rather than minima for integral values of the Landau filling factor in measurements of the Shubnikov–de Haas oscillations, thus the term "integral quantum Hall effect". These oscillations show a phase shift of π, known as Berry's phase.[32][73] Berry's phase arises due to chirality or dependence (locking) of the pseudospin quantum number on the momentum of low-energy electrons near the Dirac points.[34] The temperature dependence of the oscillations reveals that the carriers have a non-zero cyclotron mass, despite their zero effective mass in the Dirac-fermion formalism.[32]

#### Experimental observations

Graphene samples prepared on nickel films, and on both the silicon face and carbon face of silicon carbide, show the anomalous effect directly in electrical measurements.[96][97][98][99][100][101] Graphitic layers on the carbon face of silicon carbide show a clear Dirac spectrum in angle-resolved photoemission experiments, and the effect is observed in cyclotron resonance and tunneling experiments.[102]

### "Massive" electrons

Graphene's unit cell has two identical carbon atoms and two zero-energy states: one where the electron resides on atom A, and the other on atom B. However, if the unit cell's two atoms are not identical, the situation changes. Research shows that placing hexagonal boron nitride (h-BN) in contact with graphene can alter the potential felt at atoms A and B sufficiently for the electrons to develop a mass and an accompanying band gap of about 30 meV.[103]

The mass can be positive or negative. An arrangement that slightly raises the energy of an electron on atom A relative to atom B gives it a positive mass, while an arrangement that raises the energy of atom B produces a negative electron mass. The two versions behave alike and are indistinguishable via optical spectroscopy. An electron traveling from a positive-mass region to a negative-mass region must cross an intermediate region where its mass once again becomes zero. This region is gapless and therefore metallic. Metallic modes bounding semiconducting regions of opposite-sign mass is a hallmark of a topological phase and displays much the same physics as topological insulators.[103]

If the mass in graphene can be controlled, electrons can be confined to massless regions by surrounding them with massive regions, allowing the patterning of quantum dots, wires, and other mesoscopic structures. It also produces one-dimensional conductors along the boundary. These wires would be protected against backscattering and could carry currents without dissipation.[103]

### Inertial effect and kinetic inductance

While a single electron exhibits zero effective mass in graphene, as the entire set of electrons is moved with an electric field, the Fermi disk shifts, with both the total kinetic energy E and the magnitude of the total momentum P being increased. Since E is minimum when P=0, to the first order, E∼P2 must hold.[104] The proportional constant must be given by 1/(2M) where M is the collective mass (inertia) of graphene electrons. Another view of this is to associate the total kinetic energy with the current. Because the total momentum is proportional to the current I, E∼I2 must hold. The proportional constant must be given by (1/2)Lk, where Lk is a quantity of inductance unit, but its origin is not the Faraday induction but the inertial effect. Lk is the graphene kinetic inductance,[104] and is given by LK=(πℏ2)/(e2ϵFW) per unit length for a graphene strip with a width W (ϵF is the Fermi energy). The kinetic inductance, representing the collective inertial effect, is intimately linked to graphene plasmonics, and was directly measured via microwave network analysis in 2014.[104]

## Interactions and phenomena

### Strong magnetic fields

In magnetic fields above 10 tesla, additional plateaus of the Hall conductivity at σxy = νe2/h with ν = 0, ±1, ±4 are observed.[105] A plateau at ν = 3[106] and the fractional quantum Hall effect at ν = ⁠1/3⁠ were also reported.[106][107]

These observations with ν = 0, ±1, ±3, ±4 indicate that the four-fold degeneracy (two valley and two spin degrees of freedom) of the Landau energy levels is partially or completely lifted.

### Casimir effect

The Casimir effect is an interaction between disjoint neutral bodies provoked by the fluctuations of the electromagnetic vacuum. Mathematically, it can be explained by considering the normal modes of electromagnetic fields, which explicitly depend on the boundary conditions on the interacting bodies' surfaces. Due to graphene's strong interaction with the electromagnetic field as a one-atom-thick material, the Casimir effect has garnered significant interest.[108][109]

### Van der Waals force

The Van der Waals force (or dispersion force) is also unusual, obeying an inverse cubic asymptotic power law in contrast to the usual inverse quartic law.[110]

### Permittivity

Graphene's permittivity varies with frequency. Over a range from microwave to millimeter wave frequencies, it is approximately 3.3.[111] This permittivity, combined with its ability to function as both a conductor and as an insulator, theoretically allows compact capacitors made of graphene to store large amounts of electrical energy.

## Optical properties

Graphene exhibits unique optical properties, showing unexpectedly high opacity for an atomic monolayer in vacuum, absorbing approximately πα ≈ 2.3% of light from visible to infrared wavelengths,[5][6][112] where α is the fine-structure constant. This is due to the unusual low-energy electronic structure of monolayer graphene, characterized by electron and hole conical bands meeting at the Dirac point, which is qualitatively different from more common quadratic massive bands.[5] Based on the Slonczewski–Weiss–McClure (SWMcC) band model of graphite, calculations using Fresnel equations in the thin-film limit account for interatomic distance, hopping values, and frequency, thus assessing optical conductance.

Experimental verification, though confirmed, lacks the precision required to improve upon existing techniques for determining the fine-structure constant.[113]

### Multi-parametric surface plasmon resonance

Multi-parametric surface plasmon resonance has been utilized to characterize both the thickness and refractive index of chemical-vapor-deposition (CVD)-grown graphene films. At a wavelength of 670 nm (6.7×10−7 m), measured refractive index and extinction coefficient values are 3.135 and 0.897, respectively. Thickness determination yielded 3.7 Å across a 0.5mm area, consistent with the 3.35 Å reported for layer-to-layer carbon atom distance of graphite crystals.[114] This method is applicable for real-time label-free interactions of graphene with organic and inorganic substances. The existence of unidirectional surface plasmons in nonreciprocal graphene-based gyrotropic interfaces has been theoretically demonstrated, offering tunability from THz to near-infrared and visible frequencies by controlling graphene's chemical potential.[115] Particularly, the unidirectional frequency bandwidth can be 1– 2 orders of magnitude larger than that achievable with metal under similar magnetic field conditions, stemming from graphene's extremely small effective electron mass.

### Tunable band gap and optical response

Graphene's band gap can be tuned from 0 to 0.25 eV (about 5-micrometer wavelength) by applying a voltage to a dual-gate bilayer graphene field-effect transistor (FET) at room temperature.[116] The optical response of graphene nanoribbons is tunable into the terahertz regime by an applied magnetic fields.[117] Graphene/graphene oxide systems exhibit electrochromic behavior, enabling tuning of both linear and ultrafast optical properties.[118]

### Graphene-based Bragg grating

A graphene-based Bragg grating (one-dimensional photonic crystal) has been fabricated, demonstrating its capability to excite surface electromagnetic waves in periodic structure using a 633 nm (6.33×10−7 m) He–Ne laser as the light source.[119]

### Saturable absorption

Graphene exhibits unique saturable absorption, which saturates when the input optical intensity exceeds a threshold value. This nonlinear optical behavior, termed saturable absorption, occurs across the visible to near-infrared spectrum, due to graphene's universal optical absorption and zero band gap. This property has enabled full-band mode-locking in fiber lasers using graphene-based saturable absorbers, contributing significantly to ultrafast photonics. Additionally, the optical response of graphene/graphene oxide layers can be electrically tuned.[118][120][121][122][123][124]

Saturable absorption in graphene could occur at the Microwave and Terahertz band, owing to its wideband optical absorption property. The microwave-saturable absorption in graphene demonstrates the possibility of graphene microwaves and terahertz photonics devices, such as a microwave-saturable absorber, modulator, polarizer, microwave signal processing, and broadband wireless access networks.[125]

### Nonlinear Kerr effect

Under intense laser illumination, graphene exhibits a nonlinear phase shift due to the optical nonlinear Kerr effect. Graphene demonstrates a large nonlinear Kerr coefficient of 10−7 cm2⋅W−1, nearly nine orders of magnitude larger than that of bulk dielectrics,[126] suggesting its potential as a powerful nonlinear Kerr medium capable of supporting various nonlinear effects, including solitons.[127]

## Excitonic properties

First-principle calculations incorporating quasiparticle corrections and many-body effects have been employed to study the electronic and optical properties of graphene-based materials. The approach was described as three stages.[128] With GW calculation, the properties of graphene-based materials were accurately investigated, including bulk graphene,[129] nanoribbons,[130] edge and surface functionalized armchair ribbons,[131] hydrogen saturated armchair ribbons,[132] Josephson effect in graphene SNS junctions with single localized defect[133] and armchair ribbon scaling properties.[134]

### Spin transport

Graphene is considered an ideal material for spintronics due to its minimal spin–orbit interaction, the near absence of nuclear magnetic moments in carbon, and weak hyperfine interaction. Electrical injection and detection of spin current have been demonstrated up to room temperature,[135][136][137] with spin coherence length exceeding 1 micrometer observed at this temperature.[135] Control of spin current polarity via electrical gating has been achieved at low temperatures.[136]

## Magnetic properties

### Strong magnetic fields

Graphene's quantum Hall effect in magnetic fields above approximately 10 tesla reveals additional interesting features. Additional plateaus in Hall conductivity at σxy=νe2/h with ν=0,±1,±4 have been observed,[105] along with plateau at ν=3[106] and a fractional quantum Hall effect at ν=1/3.[106][107]

### Spintronic properties

Graphene exhibits spintronic and magnetic properties concurrently.[138] Low-defect graphene Nano-meshes, fabricated using a non-lithographic approach, exhibit significant ferromagnetism even at room temperature. Additionally, a spin pumping effect has been observed with fields applied in parallel to the planes of few-layer ferromagnetic nano-meshes, while a magnetoresistance hysteresis loop is evident under perpendicular fields. Charge-neutral graphene has demonstrated magnetoresistance exceeding 100% in magnetic fields generated by standard permanent magnets (approximately 0.1 tesla), marking a record magneto resistivity at room temperature among known materials.[139]

### Magnetic substrates

In 2010, researchers magnetized graphene by producing it via CVD on the Ni(111) substrate[140] and then in 2014 by placing it on an atomically smooth layer of magnetic yttrium iron garnet, maintaining graphene's electronic properties unaffected. Previous methods involved doping graphene with other substances.[141] The dopant's presence negatively affected its electronic properties.[142]

## Mechanical properties

As noted above, the (two-dimensional) density of graphene is 0.762 mg per square meter.

Graphene is the strongest material ever tested,[7][8] with an intrinsic tensile strength of 130 GPa (19,000,000 psi) (with representative engineering tensile strength ~50-60 GPa for stretching large-area freestanding graphene) and a Young's modulus (stiffness) close to 1 TPa (150,000,000 psi). The Nobel announcement illustrated this by saying that a 1 square meter graphene hammock would support a 4 kg cat but would weigh only as much as one of the cat's whiskers, at 0.77 mg (about 0.001% of the weight of 1 m2 of paper).[143]

Large-angle bending of graphene monolayers with minimal strain demonstrates its mechanical robustness. Even under extreme deformation, monolayer graphene maintains excellent carrier mobility.[144]

The spring constant of suspended graphene sheets has been measured using an atomic force microscope (AFM). Graphene sheets were suspended over SiO2 cavities where an AFM tip was used to apply stress to the sheet to test its mechanical properties. Its spring constant was in the range 1–5 N/m and the stiffness was 0.5 TPa, which differs from that of bulk graphite. These intrinsic properties could lead to applications such as NEMS as pressure sensors and resonators.[145] Due to its large surface energy and out of plane ductility, flat graphene sheets are unstable with respect to scrolling, i.e. bending into a cylindrical shape, which is its lower-energy state.[146]

In two-dimensional structures like graphene, thermal and quantum fluctuations cause relative displacement, with fluctuations growing logarithmically with structure size as per the Mermin–Wagner theorem. This shows that the amplitude of long-wavelength fluctuations grows logarithmically with the scale of a 2D structure, and would therefore be unbounded in structures of infinite size. Local deformation and elastic strain are negligibly affected by this long-range divergence in relative displacement. It is believed that a sufficiently large 2D structure, in the absence of applied lateral tension, will bend and crumple to form a fluctuating 3D structure. Researchers have observed ripples in suspended layers of graphene,[36] and it has been proposed that the ripples are caused by thermal fluctuations in the material. As a consequence of these dynamical deformations, it is debatable whether graphene is truly a 2D structure.[2][67][68][147][148] These ripples, when amplified by vacancy defects, induce a negative Poisson's ratio into graphene, resulting in the thinnest auxetic material known so far.[149]

Graphene-nickel (Ni) composites, created through plating processes, exhibit enhanced mechanical properties due to strong Ni-graphene interactions inhibiting dislocation sliding in the Ni matrix.[150]

### Fracture toughness

In 2014, researchers from Rice University and the Georgia Institute of Technology have indicated that despite its strength, graphene is also relatively brittle, with a fracture toughness of about 4 MPa√m.[151] This indicates that imperfect graphene is likely to crack in a brittle manner like ceramic materials, as opposed to many metallic materials which tend to have fracture toughness in the range of 15–50 MPa√m. Later in 2014, the Rice team announced that graphene showed a greater ability to distribute force from an impact than any known material, ten times that of steel per unit weight.[152] The force was transmitted at 22.2 kilometres per second (13.8 mi/s).[153]

### Polycrystalline graphene

Various methods – most notably, chemical vapor deposition (CVD), as discussed in the section below – have been developed to produce large-scale graphene needed for device applications. Such methods often synthesize polycrystalline graphene.[154] The mechanical properties of polycrystalline graphene are affected by the nature of the defects, such as grain-boundaries (GB) and vacancies, present in the system and the average grain-size.

Graphene grain boundaries typically contain heptagon-pentagon pairs. The arrangement of such defects depends on whether the GB is in a zig-zag or armchair direction. It further depends on the tilt-angle of the GB.[155] In 2010, researchers from Brown University computationally predicted that as the tilt-angle increases, the grain boundary strength also increases. They showed that the weakest link in the grain boundary is at the critical bonds of the heptagon rings. As the grain boundary angle increases, the strain in these heptagon rings decreases, causing the grain boundary to be stronger than lower-angle GBs. They proposed that, in fact, for sufficiently large angle GB, the strength of the GB is similar to pristine graphene.[156] In 2012, it was further shown that the strength can increase or decrease, depending on the detailed arrangements of the defects.[157] These predictions have since been supported by experimental evidence. In a 2013 study led by James Hone's group, researchers probed the elastic stiffness and strength of CVD-grown graphene by combining nano-indentation and high-resolution TEM. They found that the elastic stiffness is identical and strength is only slightly lower than those in pristine graphene.[158] In the same year, researchers from University of California, Berkeley and University of California, Los Angeles probed bi-crystalline graphene with TEM and AFM. They found that the strength of grain boundaries indeed tends to increase with the tilt angle.[159]

While the presence of vacancies is not only prevalent in polycrystalline graphene, vacancies can have significant effects on the strength of graphene. The consensus is that the strength decreases along with increasing densities of vacancies. Various studies have shown that for graphene with a sufficiently low density of vacancies, the strength does not vary significantly from that of pristine graphene. On the other hand, a high density of vacancies can severely reduce the strength of graphene.[160]

Compared to the fairly well-understood nature of the effect that grain boundary and vacancies have on the mechanical properties of graphene, there is no clear consensus on the general effect that the average grain size has on the strength of polycrystalline graphene.[161][160][162] In fact, three notable theoretical or computational studies on this topic have led to three different conclusions.[163][164][165] First, in 2012, Kolakowski and Myer studied the mechanical properties of polycrystalline graphene with "realistic atomistic model", using molecular-dynamics (MD) simulation. To emulate the growth mechanism of CVD, they first randomly selected nucleation sites that are at least 5A (arbitrarily chosen) apart from other sites. Polycrystalline graphene was generated from these nucleation sites and was subsequently annealed at 3000K, and then quenched. Based on this model, they found that cracks are initiated at grain-boundary junctions, but the grain size does not significantly affect the strength.[163] Second, in 2013, Z. Song et al. used MD simulations to study the mechanical properties of polycrystalline graphene with uniform-sized hexagon-shaped grains. The hexagon grains were oriented in various lattice directions and the GBs consisted of only heptagon, pentagon, and hexagonal carbon rings. The motivation behind such a model was that similar systems had been experimentally observed in graphene flakes grown on the surface of liquid copper. While they also noted that crack is typically initiated at the triple junctions, they found that as the grain size decreases, the yield strength of graphene increases. Based on this finding, they proposed that polycrystalline follows pseudo Hall-Petch relationship.[164] Third, in 2013, Z. D. Sha et al. studied the effect of grain size on the properties of polycrystalline graphene, by modeling the grain patches using Voronoi construction. The GBs in this model consisted of heptagons, pentagons, and hexagons, as well as squares, octagons, and vacancies. Through MD simulation, contrary to the aforementioned study, they found an inverse Hall-Petch relationship, where the strength of graphene increases as the grain size increases.[165] Experimental observations and other theoretical predictions also gave differing conclusions, similar to the three given above.[162] Such discrepancies show the complexity of the effects that grain size, arrangements of defects, and the nature of defects have on the mechanical properties of polycrystalline graphene.

## Other properties

### Thermal conductivity

Thermal transport in graphene is a burgeoning area of research, particularly for its potential applications in thermal management. Most experimental measurements have posted large uncertainties in the results of thermal conductivity due to the limitations of the instruments used. Following predictions for graphene and related carbon nanotubes,[166] early measurements of the thermal conductivity of suspended graphene reported an exceptionally large thermal conductivity up to 5300 W⋅m−1⋅K−1,[167] compared with the thermal conductivity of pyrolytic graphite of approximately 2000 W⋅m−1⋅K−1 at room temperature.[168] However, later studies primarily on more scalable but more defected graphene derived by Chemical Vapor Deposition have been unable to reproduce such high thermal conductivity measurements, producing a wide range of thermal conductivities between 1500 – 2500 W⋅m−1⋅K−1 for suspended single-layer graphene.[169][170][171][172] The large range in the reported thermal conductivity can be caused by large measurement uncertainties as well as variations in the graphene quality and processing conditions. In addition, it is known that when single-layer graphene is supported on an amorphous material, the thermal conductivity is reduced to about 500 – 600 W⋅m−1⋅K−1 at room temperature as a result of scattering of graphene lattice waves by the substrate,[173][174] and can be even lower for few-layer graphene encased in amorphous oxide.[175] Likewise, polymeric residue can contribute to a similar decrease in the thermal conductivity of suspended graphene to approximately 500 – 600 W⋅m−1⋅K−1 for bilayer graphene.[176]

Isotopic composition, specifically the ratio of 12C to 13C, significantly affects graphene's thermal conductivity. Isotopically pure 12C graphene exhibits higher thermal conductivity than either a 50:50 isotope ratio or the naturally occurring 99:1 ratio.[177] It can be shown by using the Wiedemann–Franz law, that the thermal conduction is phonon-dominated.[167] However, for a gated graphene strip, an applied gate bias causing a Fermi energy shift much larger than kBT can cause the electronic contribution to increase and dominate over the phonon contribution at low temperatures. The ballistic thermal conductance of graphene is isotropic.[178][179]

Graphite, a 3D counterpart to graphene, exhibits a basal plane thermal conductivity exceeding 1000 W⋅m−1⋅K−1 (similar to diamond), In graphite, the c-axis (out of plane) thermal conductivity is over a factor of ~100 smaller due to the weak binding forces between basal planes as well as the larger lattice spacing.[180] In addition, the ballistic thermal conductance of graphene is shown to give the lower limit of the ballistic thermal conductance, per unit circumference, length of carbon nanotubes.[181]

Graphene's thermal conductivity is influenced by its three acoustic phonon modes: two linear dispersion relation dispersion relation in-plane modes (LA, TA) and one quadratic dispersion relation out-of-plane mode (ZA). At low temperatures, the dominance of the T1.5 thermal conductivity contribution of the out-of-plane mode supersedes the T2 dependence of the linear modes.[181] Some graphene phonon bands exhibit negative Grüneisen parameters,[182] resulting in negative thermal expansion coefficient at low temperatures. The lowest negative Grüneisen parameters correspond to the lowest transverse acoustic ZA modes, whose frequencies increase with in-plane lattice parameter, akin to a stretched string with higher frequency vibrations.[183]

### Chemical properties

Graphene has a theoretical specific surface area (SSA) of 2630 m2/g. This is much larger than that reported to date for carbon black (typically smaller than 900 m2/g) or for carbon nanotubes (CNTs), from ≈100 to 1000 m2/g and is similar to activated carbon.[184] Graphene is the only form of carbon (or solid material) in which every atom is available for chemical reaction from two sides (due to the 2D structure). Atoms at the edges of a graphene sheet have special chemical reactivity. Graphene has the highest ratio of edge atoms of any allotrope. Defects within a sheet increase its chemical reactivity.[185] The onset temperature of reaction between the basal plane of single-layer graphene and oxygen gas is below 260 °C (530 K).[186] Graphene burns at very low temperatures (e.g., 350 °C (620 K)).[187] Graphene is commonly modified with oxygen- and nitrogen-containing functional groups and analyzed by infrared spectroscopy and X-ray photoelectron spectroscopy. However, the determination of structures of graphene with oxygen-[188] and nitrogen-[189] functional groups require the structures to be well controlled.

In 2013, Stanford University physicists reported that single-layer graphene is a hundred times more chemically reactive than thicker multilayer sheets.[190]

Graphene can self-repair holes in its sheets, when exposed to molecules containing carbon, such as hydrocarbons. Bombarded with pure carbon atoms, the atoms perfectly align into hexagons, filling the holes.[191][192]

### Biological properties

Despite the promising results in different cell studies and proof of concept studies, there is still incomplete understanding of the full biocompatibility of graphene-based materials.[193] Different cell lines react differently when exposed to graphene, and it has been shown that the lateral size of the graphene flakes, the form and surface chemistry can elicit different biological responses on the same cell line.[194]

There are indications that graphene has promise as a useful material for interacting with neural cells; studies on cultured neural cells show limited success.[195][196]

Graphene also has some utility in osteogenesis. Researchers at the Graphene Research Centre at the National University of Singapore (NUS) discovered in 2011 the ability of graphene to accelerate the osteogenic differentiation of human mesenchymal stem cells without the use of biochemical inducers.[197]

Graphene can be used in biosensors; in 2015, researchers demonstrated that a graphene-based sensor can be used to detect a cancer risk biomarker. In particular, by using epitaxial graphene on silicon carbide, they were repeatedly able to detect 8-hydroxydeoxyguanosine (8-OHdG), a DNA damage biomarker.[198]

### Support substrate

The electronic property of graphene can be significantly influenced by the supporting substrate. Studies of graphene monolayers on clean and hydrogen(H)-passivated silicon (100) (Si(100)/H) surfaces have been performed.[199] The Si(100)/H surface does not perturb the electronic properties of graphene, whereas the interaction between the clean Si(100) surface and graphene changes the electronic states of graphene significantly. This effect results from the covalent bonding between C and surface Si atoms, modifying the π-orbital network of the graphene layer. The local density of states shows that the bonded C and Si surface states are highly disturbed near the Fermi energy.

## Graphene layers and structural variants

### Monolayer sheets

In 2013 a group of Polish scientists presented a production unit that allows the manufacture of continuous monolayer sheets.[200] The process is based on graphene growth on a liquid metal matrix.[201] The product of this process was called High Strength Metallurgical Graphene. In a new study published in Nature, the researchers have used a single-layer graphene electrode and a novel surface-sensitive non-linear spectroscopy technique to investigate the top-most water layer at the electrochemically charged surface. They found that the interfacial water response to the applied electric field is asymmetric concerning the nature of the applied field.[202]

### Bilayer graphene

Main article: Physics:Bilayer graphene

Bilayer graphene displays the anomalous quantum Hall effect, a tunable band gap[203] and potential for excitonic condensation[204] –making it a promising candidate for optoelectronic and nanoelectronic applications. Bilayer graphene typically can be found either in twisted configurations where the two layers are rotated relative to each other or graphitic Bernal stacked configurations where half the atoms in one layer lie atop half the atoms in the other.[205] Stacking order and orientation govern the optical and electronic properties of bilayer graphene.

One way to synthesize bilayer graphene is via chemical vapor deposition, which can produce large bilayer regions that almost exclusively conform to a Bernal stack geometry.[205]

It has been shown that the two graphene layers can withstand important strain or doping mismatch[206] which ultimately should lead to their exfoliation.

### Turbostratic

Turbostratic graphene exhibits weak interlayer coupling, and the spacing is increased with respect to Bernal-stacked multilayer graphene. Rotational misalignment preserves the 2D electronic structure, as confirmed by Raman spectroscopy.[207] The D peak is very weak, whereas the 2D and G peaks remain prominent.[207]

A rather peculiar feature is that the I2D/IG ratio can exceed 10. However, most importantly, the M peak, which originates from AB stacking, is absent, whereas the TS1 and TS2 modes are visible in the Raman spectrum.[208][209] The material is formed through conversion of non-graphenic carbon into graphenic carbon without providing sufficient energy to allow for the reorganization through annealing of adjacent graphene layers into crystalline graphitic structures.

### Graphene superlattices

Periodically stacked graphene and its insulating isomorph provide a fascinating structural element in implementing highly functional superlattices at the atomic scale, which offers possibilities for designing nanoelectronic and photonic devices. Various types of superlattices can be obtained by stacking graphene and its related forms.[210] The energy band in layer-stacked superlattices is found to be more sensitive to the barrier width than that in conventional III–V semiconductor superlattices. When adding more than one atomic layer to the barrier in each period, the coupling of electronic wavefunctions in neighboring potential wells can be significantly reduced, which leads to the degeneration of continuous subbands into quantized energy levels. When varying the well width, the energy levels in the potential wells along the L-M direction behave distinctly from those along the K-H direction.

A superlattice corresponds to a periodic or quasi-periodic arrangement of different materials and can be described by a superlattice period which confers a new translational symmetry to the system, impacting their phonon dispersions and subsequently their thermal transport properties. Recently, uniform monolayer graphene-hBN structures have been successfully synthesized via lithography patterning coupled with chemical vapor deposition (CVD).[211] Furthermore, superlattices of graphene-HBN are ideal model systems for the realization and understanding of coherent (wave-like) and incoherent (particle-like) phonon thermal transport.[212][213][214][215][216]

## Nanostructured graphene forms

### Graphene nanoribbons

Names for graphene edge topologies GNR Electronic band structure of graphene strips of varying widths in zig-zag orientation. Tight-binding calculations show that they are all metallic. GNR Electronic band structure of graphene strips of various widths in the armchair orientation. Tight-binding calculations show that they are semiconducting or metallic depending on width (chirality).

Graphene nanoribbons ("nanostripes" in the "zig-zag"/"zigzag" orientation), at low temperatures, show spin-polarized metallic edge currents, which also suggests applications in the new field of spintronics. (In the "armchair" orientation, the edges behave like semiconductors.[72])

### Graphene quantum dots

A graphene quantum dot (GQD) is a graphene fragment with a size lesser than 100 nm. The properties of GQDs are different from bulk graphene due to the quantum confinement effects which only become apparent when the size is smaller than 100 nm.[217][218][219]

## Modified and functionalized graphene

Main article: Chemistry:Graphene chemistry

### Graphene oxide

Graphene oxide is usually produced through chemical exfoliation of graphite. A particularly popular technique is the improved Hummers' method.[220] Using paper-making techniques on dispersed, oxidized and chemically processed graphite in water, the monolayer flakes form a single sheet and create strong bonds. These sheets, called graphene oxide paper, have a measured tensile modulus of 32 GPa.[221] The chemical property of graphite oxide is related to the functional groups attached to graphene sheets. These can change the polymerization pathway and similar chemical processes.[222] Graphene oxide flakes in polymerss display enhanced photo-conducting properties.[223] Graphene is normally hydrophobic and impermeable to all gases and liquids (vacuum-tight). However, when formed into a graphene oxide-based capillary membrane, both liquid water and water vapor flow through as quickly as if the membrane were not present.[224]

In 2022, researchers evaluated the biological effects of low doses on graphene oxide on larvae and imago of Drosophila melanogaster. Results show that oral administration of graphene oxide at concentrations of 0.02-1% has a beneficial effect on the developmental rate and hatching ability of larvae. Long-term administration of a low dose of graphene oxide extends the lifespan of Drosophila and significantly enhances resistance to environmental stresses. These suggest that graphene oxide affects carbohydrate and lipid metabolism in adult Drosophila. These findings might provide a useful reference to assess the biological effects of graphene oxide, which could play an important role in a variety of graphene-based biomedical applications.[225]

### Chemical modification

Photograph of single-layer graphene oxide undergoing high temperature chemical treatment, resulting in sheet folding and loss of carboxylic functionality, or through room temperature carbodiimide treatment, collapsing into star-like clusters.

Soluble fragments of graphene can be prepared in the laboratory through chemical modification of graphite.[226] First, microcrystalline graphite is treated with an acidic mixture of sulfuric acid and nitric acid. A series of oxidation and exfoliation steps produce small graphene plates with carboxyl groups at their edges. These are converted to acid chloride groups by treatment with thionyl chloride; next, they are converted to the corresponding graphene amide via treatment with octadecyl amine. The resulting material (circular graphene layers of 5.3 Å or 5.3×10−10 m thickness) is soluble in tetrahydrofuran, tetrachloromethane and dichloroethane.

Refluxing single-layer graphene oxide (SLGO) in solvents leads to size reduction and folding of individual sheets as well as loss of carboxylic group functionality, by up to 20%, indicating thermal instabilities of SLGO sheets dependent on their preparation methodology. When using thionyl chloride, acyl chloride groups result, which can then form aliphatic and aromatic amides with a reactivity conversion of around 70–80%.

Boehm titration results for various chemical reactions of single-layer graphene oxide, which reveal reactivity of the carboxylic groups and the resultant stability of the SLGO sheets after treatment.

Hydrazine reflux is commonly used for reducing SLGO to SLG(R), but titrations show that only around 20–30% of the carboxylic groups are lost, leaving a significant number available for chemical attachment. Analysis of SLG(R) generated by this route reveals that the system is unstable and using a room temperature stirring with hydrochloric acid (< 1.0 M) leads to around 60% loss of COOH functionality. Room temperature treatment of SLGO with carbodiimides leads to the collapse of the individual sheets into star-like clusters that exhibited poor subsequent reactivity with amines (c. 3–5% conversion of the intermediate to the final amide).[227] It is apparent that conventional chemical treatment of carboxylic groups on SLGO generates morphological changes of individual sheets that leads to a reduction in chemical reactivity, which may potentially limit their use in composite synthesis. Therefore, chemical reaction types have been explored. SLGO has also been grafted with polyallylamine, cross-linked through epoxy groups. When filtered into graphene oxide paper, these composites exhibit increased stiffness and strength relative to unmodified graphene oxide paper.[228]

Full hydrogenation from both sides of the graphene sheet results in Graphane, but partial hydrogenation leads to hydrogenated graphene.[229] Similarly, both-side fluorination of graphene (or chemical and mechanical exfoliation of graphite fluoride) leads to fluorographene (graphene fluoride),[230] while partial fluorination (generally halogenation) provides fluorinated (halogenated) graphene.

### Graphene ligand/complex

Graphene can be a ligand to coordinate metals and metal ions by introducing functional groups. Structures of graphene ligands are similar to e.g. metal-porphyrin complex, metal-phthalocyanine complex, and metal-phenanthroline complex. Copper and nickel ions can be coordinated with graphene ligands.[231][232]

## Advanced graphene structures

### Graphene fiber

In 2011, researchers reported a novel yet simple approach to fabricating graphene fibers from chemical vapor deposition-grown graphene films.[233] The method was scalable and controllable, delivering tunable morphology and pore structure by controlling the evaporation of solvents with suitable surface tension. Flexible all-solid-state supercapacitors based on these graphene fibers were demonstrated in 2013.[234]

In 2015, intercalating small graphene fragments into the gaps formed by larger, coiled graphene sheets, after annealing provided pathways for conduction, while the fragments helped reinforce the fibers.[sentence fragment] The resulting fibers offered better thermal and electrical conductivity and mechanical strength. Thermal conductivity reached 1,290 W/m/K (1,290 watts per metre per kelvin), while tensile strength reached 1,080 MPa (157,000 psi).[235]

In 2016, kilometer-scale continuous graphene fibers with outstanding mechanical properties and excellent electrical conductivity were produced by high-throughput wet-spinning of graphene oxide liquid crystals followed by graphitization through a full-scale synergetic defect-engineering strategy.[236] The graphene fibers with superior performances promise wide applications in functional textiles, lightweight motors, microelectronic devices, etc.

Tsinghua University in Beijing, led by Wei Fei of the Department of Chemical Engineering, claims to be able to create a carbon nanotube fiber that has a tensile strength of 80 GPa (12,000,000 psi).[237]

### 3D graphene

In 2013, a three-dimensional honeycomb of hexagonally arranged carbon was termed 3D graphene, and self-supporting 3D graphene was also produced.[238] 3D structures of graphene can be fabricated by using either CVD or solution-based methods. A 2016 review by Khurram and Xu et al. provided a summary of then-state-of-the-art techniques for fabrication of the 3D structure of graphene and other related two-dimensional materials.[239] In 2013, researchers at Stony Brook University reported a novel radical-initiated crosslinking method to fabricate porous 3D free-standing architectures of graphene and carbon nanotubes using nanomaterials as building blocks without any polymer matrix as support.[240] These 3D graphenes (all-carbon) scaffolds/foams have applications in several fields such as energy storage, filtration, thermal management, and biomedical devices and implants.[239][241]

Box-shaped graphene (BSG) nanostructure appearing after mechanical cleavage of pyrolytic graphite was reported in 2016.[242] The discovered nanostructure is a multilayer system of parallel hollow nanochannels located along the surface and having quadrangular cross-section. The thickness of the channel walls is approximately equal to 1 nm. Potential fields of BSG application include ultra-sensitive detectors, high-performance catalytic cells, nanochannels for DNA sequencing and manipulation, high-performance heat sinking surfaces, rechargeable batteries of enhanced performance, nanomechanical resonators, electron multiplication channels in emission Nano-electronic devices, high-capacity sorbents for safe hydrogen storage.

Three dimensional bilayer graphene has also been reported.[243][244]

### Pillared graphene

Main article: Chemistry:Pillared graphene

Pillared graphene is a hybrid carbon structure, consisting of an oriented array of carbon nanotubes connected at each end to a sheet of graphene. It was first described theoretically by George Froudakis and colleagues at the University of Crete in Greece in 2008. Pillared graphene has not yet been synthesized in the laboratory, but it has been suggested that it may have useful electronic properties, or as a hydrogen storage material.

### Reinforced graphene

Graphene reinforced with embedded carbon nanotube reinforcing bars ("rebar") is easier to manipulate, while improving the electrical and mechanical qualities of both materials.[245][246]

Functionalized single- or multi-walled carbon nanotubes are spin-coated on copper foils and then heated and cooled, using the nanotubes themselves as the carbon source. Under heating, the functional carbon groups decompose into graphene, while the nanotubes partially split and form in-plane covalent bonds with the graphene, adding strength. π–π stacking domains add more strength. The nanotubes can overlap, making the material a better conductor than standard CVD-grown graphene. The nanotubes effectively bridge the grain boundaries found in conventional graphene. The technique eliminates the traces of substrate on which later-separated sheets were deposited using epitaxy.[245]

Stacks of a few layers have been proposed as a cost-effective and physically flexible replacement for indium tin oxide (ITO) used in displays and photovoltaic cells.[245]

### Molded graphene

In 2015, researchers from the University of Illinois at Urbana–Champaign (UIUC) developed a new approach for forming 3D shapes from flat, 2D sheets of graphene.[247] A film of graphene that had been soaked in solvent to make it swell and become malleable was overlaid on an underlying substrate "former". The solvent evaporated over time, leaving behind a layer of graphene that had taken on the shape of the underlying structure. In this way, they were able to produce a range of relatively intricate micro-structured shapes.[248] Features vary from 3.5 to 50 μm. Pure graphene and gold-decorated graphene were each successfully integrated with the substrate.[249]

## Specialized graphene configurations

### Graphene aerogel

An aerogel made of graphene layers separated by carbon nanotubes was measured at 0.16 milligrams per cubic centimeter. A solution of graphene and carbon nanotubes in a mold is freeze-dried to dehydrate the solution, leaving the aerogel. The material has superior elasticity and absorption. It can recover completely after more than 90% compression, and absorb up to 900 times its weight in oil, at a rate of 68.8 grams per second.[250]

### Graphene nanocoil

In 2015, a coiled form of graphene was discovered in graphitic carbon (coal). The spiraling effect is produced by defects in the material's hexagonal grid that causes it to spiral along its edge, mimicking a Riemann surface, with the graphene surface approximately perpendicular to the axis. When voltage is applied to such a coil, current flows around the spiral, producing a magnetic field. The phenomenon applies to spirals with either zigzag or armchair patterns, although with different current distributions. Computer simulations indicated that a conventional spiral inductor of 205 microns in diameter could be matched by a nanocoil just 70 nanometers wide, with a field strength reaching as much as 1 tesla.[251]

The nano-solenoids analyzed through computer models at Rice University should be capable of producing powerful magnetic fields of about 1 tesla, about the same as the coils found in typical loudspeakers, according to Yakobson and his team – and about the same field strength as some MRI machines. They found the magnetic field would be strongest in the hollow, nanometer-wide cavity at the spiral's center.[251]

A solenoid made with such a coil behaves as a quantum conductor whose current distribution between the core and exterior varies with applied voltage, resulting in nonlinear inductance.[252]

### Crumpled graphene

In 2016, Brown University introduced a method for "crumpling" graphene, adding wrinkles to the material on a nanoscale. This was achieved by depositing layers of graphene oxide onto a shrink film, then shrunken, with the film dissolved before being shrunken again on another sheet of film. The crumpled graphene became superhydrophobic, and when used as a battery electrode, the material was shown to have as much as a 400% increase in electrochemical current density.[253][254]

## Mechanical synthesis

Main article: Chemistry:Graphene production techniques

A rapidly increasing list of production techniques have been developed to enable graphene's use in commercial applications.[255]

Isolated 2D crystals cannot be grown via chemical synthesis beyond small sizes even in principle, because the rapid growth of phonon density with increasing lateral size forces 2D crystallites to bend into the third dimension. In all cases, graphene must bond to a substrate to retain its two-dimensional shape.[19]

### Bottom-up and top-down methods

Small graphene structures, such as graphene quantum dots and nanoribbons, can be produced by "bottom-up" methods that assemble the lattice from organic molecule monomers (e. g. citric acid, glucose). "Top-down" methods, on the other hand, cut bulk graphite and graphene materials with strong chemicals (e. g. mixed acids).[256]

### Micro-mechanical cleavage

The most famous, clean and rather straightforward method of isolating graphene sheets, called micro-mechanical cleavage or more colloquially called the scotch tape method, was introduced by Novoselov et al. in 2004, which uses adhesive tape to mechanically cleave high-quality graphite crystals into successively thinner platelets. Other methods do exist like exfoliation.[256]

### Exfoliation techniques

#### Mechanical exfoliation

Geim and Novoselov initially used adhesive tape to pull graphene sheets away from graphite. Achieving single layers typically requires multiple exfoliation steps. After exfoliation, the flakes are deposited on a silicon wafer. Crystallites larger than 1 mm and visible to the naked eye can be obtained.[257]

As of 2014, exfoliation produced graphene with the lowest number of defects and highest electron mobility. One specific exfoliation technique involved using a sharp single-crystal diamond wedge to penetrate the graphite source and precisely cleave individual layers. That same year, researchers also developed liquid-phase methods, creating defect-free, unoxidized graphene-containing liquids from graphite using mixers that generate extremely high local shear rates greater than 10×104.[258][259]

A 2014 study published in Nature Materials demonstrated that scalable production of defect-free graphene is possible through shear exfoliation using a high-shear mixer. This technique can produce large quantities of few-layer graphene in solution while preserving structural integrity.[260] As turbulence is not necessary for mechanical exfoliation, resonant acoustic mixing or low-speed ball milling can also be effective in the production of high-yield and water-soluble graphene.[261][262]

#### Liquid phase exfoliation

Liquid phase exfoliation (LPE) is a relatively simple method that involves dispersing graphite in a liquid medium to produce graphene by sonication or high shear mixing, followed by centrifugation. Restacking is an issue with this technique unless solvents with appropriate surface energy are used (e.g. NMP). Adding a surfactant to a solvent prior to sonication prevents restacking by adsorbing to the graphene's surface. This produces a higher graphene concentration, but removing the surfactant requires chemical treatments.[263][264]

LPE results in nanosheets with a broad size distribution and thicknesses roughly in the range of 1-10 monolayers. However, liquid cascade centrifugation can be used to size-select the suspensions and achieve monolayer enrichment.[265]

Sonicating graphite at the interface of two immiscible liquids, most notably heptane and water, produced macro-scale graphene films. The graphene sheets are adsorbed to the high-energy interface between the materials and are kept from restacking. The sheets are up to about 95% transparent and conductive.[266]

With definite cleavage parameters, the box-shaped graphene (BSG) nanostructure can be prepared on graphite crystal.[242] A major advantage of LPE is that it can be used to exfoliate many inorganic 2D materials beyond graphene, e.g. BN, MoS2, WS2.[267]

#### Exfoliation with supercritical carbon dioxide

Liquid-phase exfoliation can also be done by a less-known process of intercalating supercritical carbon dioxide (scCO2) into the interstitial spaces in the graphite lattice, followed by rapid depressurization. The scCO2 intercalates easily inside the graphite lattice at a pressure of roughly 100 atm. Carbon dioxide turns gaseous as soon as the vessel is depressurized and makes the graphite explode into few-layered graphene.[256]

This method may have multiple advantages: being non-toxic, the graphite does not have to be chemically treated in any way before the process, and the whole process can be completed in a single step as opposed to other exfoliation methods.[256]

### Splitting monolayer carbon allotropes

Graphene can be created by opening carbon nanotubes by cutting or etching.[268] In one such method, multi-walled carbon nanotubes were cut open in solution by action of potassium permanganate and sulfuric acid.[269][270] In 2014, carbon nanotube-reinforced graphene was made via spin coating and annealing functionalized carbon nanotubes.[245]

Another approach sprays buckyballs at supersonic speeds onto a substrate. The balls cracked open upon impact, and the resulting unzipped cages then bond together to form a graphene film.[271]

## Chemical synthesis

### Graphite oxide reduction

P. Boehm reported producing monolayer flakes of reduced graphene oxide in 1962.[272][273] Rapid heating of graphite oxide and exfoliation yields highly dispersed carbon powder with a few percent of graphene flakes.

Another method is the reduction of graphite oxide monolayer films, e.g. by hydrazine with annealing in argon/hydrogen with an almost intact carbon framework that allows efficient removal of functional groups. Measured charge carrier mobility exceeded 1,000 cm/Vs (10 m/Vs).[274]

Burning a graphite oxide coated DVD produced a conductive graphene film (1,738 siemens per meter) and specific surface area (1,520 square meters per gram) that was highly resistant and malleable.[275]

A dispersed reduced graphene oxide suspension was synthesized in water by a hydrothermal dehydration method without using any surfactant. The approach is facile, industrially applicable, environmentally friendly, and cost-effective. Viscosity measurements confirmed that the graphene colloidal suspension (graphene nanofluid) exhibits Newtonian behavior, with the viscosity showing a close resemblance to that of water.[276]

### Molten salts

Graphite particles can be corroded in molten salts to form a variety of carbon nanostructures including graphene.[277] Hydrogen cations, dissolved in molten lithium chloride, can be discharged on cathodically polarized graphite rods, which then intercalate, peeling graphene sheets. The graphene nanosheets produced displayed a single-crystalline structure with a lateral size of several hundred nanometers and a high degree of crystallinity and thermal stability.[278]

### Electrochemical synthesis

Electrochemical synthesis can exfoliate graphene. Varying a pulsed voltage controls thickness, flake area, and number of defects and affects its properties. The process begins by bathing the graphite in a solvent for intercalation. The process can be tracked by monitoring the solution's transparency with an LED and photodiode.[279][280]

### Hydrothermal self-assembly

Graphene has been prepared by using a sugar like glucose, fructose, etc. This substrate-free "bottom-up" synthesis is safer, simpler and more environmentally friendly than exfoliation. The method can control the thickness, ranging from monolayer to multilayer, which is known as the "Tang-Lau Method".[281][282][283][284]

### Sodium ethoxide pyrolysis

Gram-quantities were produced by the reaction of ethanol with sodium metal, followed by pyrolysis and washing with water.[285]

### Microwave-assisted oxidation

In 2012, microwave energy was reported to directly synthesize graphene in one step.[286] This approach avoids use of potassium permanganate in the reaction mixture. It was also reported that by microwave radiation assistance, graphene oxide with or without holes can be synthesized by controlling microwave time.[287] Microwave heating can dramatically shorten the reaction time from days to seconds.

Graphene can also be made by microwave assisted hydrothermal pyrolysis.[217][218]

### Thermal decomposition of silicon carbide

Heating silicon carbide (SiC) to high temperatures (1100 °C) under low pressures (c. 10−6 torr, or 10−4 Pa) reduces it to graphene.[97][98][99][100][101][288]

## Vapor deposition and growth techniques

### Chemical vapor deposition

#### Epitaxy

Epitaxial graphene growth on silicon carbide is a wafer-scale technique to produce graphene. Epitaxial graphene may be coupled to surfaces weakly enough (by the active valence electrons that create Van der Waals forces) to retain the two-dimensional electronic band structure of isolated graphene.[289]

A normal silicon wafer coated with a layer of germanium (Ge) dipped in dilute hydrofluoric acid strips the naturally forming germanium oxide groups, creating hydrogen-terminated germanium. CVD can coat that with graphene.[290][291]

The direct synthesis of graphene on insulator TiO2 with high-dielectric-constant (high-κ). A two-step CVD process is shown to grow graphene directly on TiO2 crystals or exfoliated TiO2 nanosheets without using any metal catalyst.[292]

#### Metal substrates

CVD graphene can be grown on metal substrates including ruthenium,[293] iridium,[294] nickel[295] and copper.[296][297]

#### Roll-to-roll

In 2014, a two-step roll-to-roll manufacturing process was announced. The first roll-to-roll step produces the graphene via chemical vapor deposition. The second step binds the graphene to a substrate.[298][299]

Large-area Raman mapping of CVD graphene on deposited Cu thin film on 150 mm SiO2/Si wafers reveals >95% monolayer continuity and an average value of ~2.62 for I2D/IG. The scale bar is 200 μm.

#### Cold wall

Growing graphene in an industrial resistive-heating cold wall CVD system was claimed to produce graphene 100 times faster than conventional CVD systems, cut costs by 99%, and produce material with enhanced electronic qualities.[300][301]

#### Wafer scale CVD graphene

CVD graphene is scalable and has been grown on deposited Cu thin film catalyst on 100 to 300 mm standard Si/SiO2 wafers[302][303][304] on an Axitron Black Magic system. Monolayer graphene coverage of >95% is achieved on 100 to 300 mm wafer substrates with negligible defects, confirmed by extensive Raman mapping.[303][304]

### Solvent interface trapping method (SITM)

As reported by a group led by D. H. Adamson, graphene can be produced from natural graphite while preserving the integrity of the sheets using the solvent interface trapping method (SITM). SITM uses a high-energy interface, such as oil and water, to exfoliate graphite to graphene. Stacked graphite delaminates, or spreads, at the oil/water interface to produce few-layer graphene in a thermodynamically favorable process in much the same way as small molecule surfactants spread to minimize the interfacial energy. In this way, graphene behaves like a 2D surfactant.[305][306][307] SITM has been reported for a variety of applications such conductive polymer-graphene foams,[308][309][310][311] conductive polymer-graphene microspheres,[312] conductive thin films[313] and conductive inks.[314]

### Carbon dioxide reduction

A highly exothermic reaction combusts magnesium in an oxidation-reduction reaction with carbon dioxide, producing carbon nanoparticles including graphene and fullerenes.[315]

### Supersonic spray

Supersonic acceleration of droplets through a Laval nozzle was used to deposit reduced graphene oxide on a substrate. The energy of the impact rearranges those carbon atoms into flawless graphene.[316][317]

### Laser

In 2014, a CO2 infrared laser was used to produce patterned porous three-dimensional laser-induced graphene (LIG) film networks from commercial polymer films. The resulting material exhibits high electrical conductivity and surface area. The laser induction process is compatible with roll-to-roll manufacturing processes.[318] A similar material, laser-induced graphene fibers (LIGF), was reported in 2018.[319]

### Flash Joule heating

In 2019, flash Joule heating (transient high-temperature electrothermal heating) was discovered to be a method to synthesize turbostratic graphene in bulk powder form. The method involves electrothermally converting various carbon sources, such as carbon black, coal, and food waste into micron-scale flakes of graphene.[208][320] More recent works demonstrated the use of mixed plastic waste, waste rubber tires, and pyrolysis ash as carbon feedstocks.[321][322][323] The graphenization process is kinetically controlled, and the energy dose is chosen to preserve the carbon in its graphenic state (excessive energy input leads to subsequent graphitization through annealing).

### Ion implantation

Accelerating carbon ions inside an electrical field into a semiconductor made of thin nickel films on a substrate of SiO2/Si, creates a wafer-scale (4 inches (100 mm)) wrinkle/tear/residue-free graphene layer at a relatively low temperature of 500 °C.[324][325]

### CMOS-compatible graphene

Integration of graphene in the widely employed CMOS fabrication process demands its transfer-free direct synthesis on dielectric substrates at temperatures below 500 °C. At the IEDM 2018, researchers from University of California, Santa Barbara, demonstrated a novel CMOS-compatible graphene synthesis process at 300 °C suitable for back-end-of-line (BEOL) applications.[326][327][328] The process involves pressure-assisted solid-state diffusion of carbon through a thin-film of metal catalyst. The synthesized large-area graphene films were shown to exhibit high quality (via Raman characterization) and similar resistivity values when compared with high-temperature CVD synthesized graphene films of the same cross-section down to widths of 20 nm.

## Simulation

In addition to experimental investigation of graphene and graphene-based devices, numerical modeling and simulation of graphene has also been an important research topic. The Kubo formula provides an analytic expression for the graphene's conductivity and shows that it is a function of several physical parameters including wavelength, temperature, and chemical potential.[329] Moreover, a surface conductivity model, which describes graphene as an infinitesimally thin (two-sided) sheet with a local and isotropic conductivity, has been proposed. This model permits the derivation of analytical expressions for the electromagnetic field in the presence of a graphene sheet in terms of a dyadic Green function (represented using Sommerfeld integrals) and exciting electric current.[330]

Even though these analytical models and methods can provide results for several canonical problems for benchmarking purposes, many practical problems involving graphene, such as the design of arbitrarily shaped electromagnetic devices, are analytically intractable. With the recent advances in the field of computational electromagnetics (CEM), various accurate and efficient numerical methods have become available for analysis of electromagnetic field/wave interactions on graphene sheets and/or graphene-based devices. A comprehensive summary of computational tools developed for analyzing graphene-based devices/systems is proposed.[331]

## Graphene analogs

Graphene analogs[332] (also referred to as "artificial graphene") are two-dimensional systems which exhibit similar properties to graphene. Graphene analogs have been studied intensively since the discovery of graphene in 2004. People try to develop systems in which the physics is easier to observe and manipulate than in graphene. In those systems, electrons are not always the particles that are used. They might be optical photons,[333] microwave photons,[334] plasmons,[335] microcavity polaritons,[336] or even atoms.[337] Also, the honeycomb structure in which those particles evolve can be of a different nature than carbon atoms in graphene. It can be, respectively, a photonic crystal, an array of metallic rods, metallic nanoparticles, a lattice of coupled microcavities, or an optical lattice.

## Applications

Main article: Chemistry:Potential applications of graphene

Graphene is a transparent and flexible conductor that holds great promise for various material/device applications, including solar cells,[338] light-emitting diodes (LED), integrated photonic circuit devices,[339][340] touch panels, and smart windows or phones.[341] Smartphone products with graphene touch screens are already on the market.[342]

In 2013, Head announced their new range of graphene tennis racquets.[343]

As of 2015, there is one product available for commercial use: a graphene-infused printer powder.[344] Many other uses for graphene have been proposed or are under development, in areas including electronics, biological engineering, filtration, lightweight/strong composite materials, photovoltaics and energy storage.[239][345] Graphene is often produced as a powder and as a dispersion in a polymer matrix. This dispersion is supposedly suitable for advanced composites,[346][347] paints and coatings, lubricants, oils and functional fluids, capacitors and batteries, thermal management applications, display materials and packaging, solar cells, inks and 3D-printer materials, and barriers and films.[348]

On 2 August 2016, Briggs Automative Company's new Mono model is said to be made out of graphene as the first of both a street-legal track car and a production car.[349]

In January 2018, graphene-based spiral inductors exploiting kinetic inductance at room temperature were first demonstrated at the University of California, Santa Barbara, led by Kaustav Banerjee. These inductors were predicted to allow significant miniaturization in radio-frequency integrated circuit applications.[350][351][352]

The potential of epitaxial graphene on SiC for metrology has been shown since 2010, displaying quantum Hall resistance quantization accuracy of three parts per billion in monolayer epitaxial graphene. Over the years precisions of parts-per-trillion in the Hall resistance quantization and giant quantum Hall plateaus have been demonstrated. Developments in the encapsulation and doping of epitaxial graphene have led to the commercialization of epitaxial graphene quantum resistance standards.[353]

Novel uses for graphene continue to be researched and explored. One such use is in combination with water-based epoxy resins to produce anticorrosive coatings.[354] The van der Waals nature of graphene and other two-dimensional (2D) materials also permits van der Waals heterostructures[355] and integrated circuits based on Van der Waals integration of 2D materials.[356][357]

Graphene is utilized in detecting gasses and chemicals in environmental monitoring, developing highly sensitive biosensors for medical diagnostics, and creating flexible, wearable sensors for health monitoring.[358][359] Graphene's transparency also enhances optical sensors, making them more effective in imaging and spectroscopy.[360]

## Toxicity

One review on graphene toxicity published in 2016 by Lalwani et al. summarizes the in vitro, in vivo, antimicrobial and environmental effects and highlights the various mechanisms of graphene toxicity.[361] Another review published in 2016 by Ou et al. focused on graphene-family nanomaterials (GFNs) and revealed several typical mechanisms such as physical destruction, oxidative stress, DNA damage, inflammatory response, apoptosis, autophagy, and necrosis.[362]

A 2020 study showed that the toxicity of graphene is dependent on several factors such as shape, size, purity, post-production processing steps, oxidative state, functional groups, dispersion state, synthesis methods, route and dose of administration, and exposure times.[363]

In 2014, research at Stony Brook University showed that graphene nanoribbons, graphene nanoplatelets, and graphene nano–onions are non-toxic at concentrations up to 50 μg/ml. These nanoparticles do not alter the differentiation of human bone marrow stem cells towards osteoblasts (bone) or adipocytes (fat), suggesting that at low doses, graphene nanoparticles are safe for biomedical applications.[364] In 2013, research at Brown University found that 10 μm few-layered graphene flakes can pierce cell membranes in solution. They were observed to enter initially via sharp and jagged points, allowing graphene to be internalized in the cell. The physiological effects of this remain unknown, and this remains a relatively unexplored field.[365][366]

## See also

* Chemistry:Borophene - Allotrope of boron
* Chemistry:Penta-graphene
* Chemistry:Phagraphene
* Chemistry:Plumbene - Material made up of a single layer of lead atoms
* Chemistry:Silicene - Two-dimensional allotrope of silicon

## References

1. ↑ "graphene definition, meaning – what is graphene in the British English Dictionary & Thesaurus – Cambridge Dictionaries Online". cambridge.org. http://dictionary.cambridge.org/dictionary/british/graphene.
2. ↑ 2.00 2.01 2.02 2.03 2.04 2.05 2.06 2.07 2.08 2.09 2.10 2.11 2.12 2.13 2.14 Geim, A. K.; Novoselov, K. S. (26 February 2007). "The rise of graphene". Nature Materials 6 (3): 183–191. doi:10.1038/nmat1849. PMID 17330084. Bibcode: 2007NatMa...6..183G.
3. ↑ Peres, N. M. R.; Ribeiro, R. M. (2009). "Focus on Graphene". New Journal of Physics 11 (9). doi:10.1088/1367-2630/11/9/095002. Bibcode: 2009NJPh...11i5002P.
4. ↑ Pike, Jared (2023). "Is graphene the best heat conductor ever? Purdue researchers investigate with four-phonon scattering". Purdue University Mechanical Engineering News. https://engineering.purdue.edu/ME/News/2023/is-graphene-the-best-heat-conductor-ever-purdue-researchers-investigate-with-fourphonon-scattering.
5. ↑ 5.0 5.1 5.2 5.3 Nair, R. R.; Blake, P.; Grigorenko, A. N.; Novoselov, K. S.; Booth, T. J.; Stauber, T.; Peres, N. M. R.; Geim, A. K. (6 June 2008). "Fine Structure Constant Defines Visual Transparency of Graphene". Science 320 (5881): 1308. doi:10.1126/science.1156965. PMID 18388259. Bibcode: 2008Sci...320.1308N.
6. ↑ 6.0 6.1 6.2 Zhu, Shou-En; Yuan, Shengjun; Janssen, G. C. A. M. (1 October 2014). "Optical transmittance of multilayer graphene". EPL 108 (1). doi:10.1209/0295-5075/108/17007. Bibcode: 2014EL....10817007Z.
7. ↑ 7.0 7.1 Lee, Changgu (2008). "Measurement of the Elastic Properties and Intrinsic Strength of Monolayer Graphene". Science 321 (385): 385–388. doi:10.1126/science.1157996. PMID 18635798. Bibcode: 2008Sci...321..385L.
8. ↑ 8.0 8.1 Cao, K. (2020). "Elastic straining of free-standing monolayer graphene". Nature Communications 11 (284). doi:10.1038/s41467-019-14130-0. PMID 31941941. Bibcode: 2020NatCo..11..284C.
9. ↑ "Graphene: A Complete Chemical History". 20 September 2019. https://www.acsmaterial.com/blog-detail/graphene-a-complete-chemical-history.html. "In 1947, the existence of graphene was theorized by Philip R Wallace as an attempt to understand electronic properties of 3D graphite. He did not use the term "graphene", but instead referred to it as a "single hexagonal layer.""
10. ↑ 10.0 10.1 Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; Zhang, Y.; Dubonos, S. V.; Grigorieva, I. V.; Firsov, A. A. (22 October 2004). "Electric Field Effect in Atomically Thin Carbon Films". Science 306 (5696): 666–669. doi:10.1126/science.1102896. PMID 15499015. Bibcode: 2004Sci...306..666N.
11. ↑ 11.0 11.1 "This Month in Physics History: October 22, 2004: Discovery of Graphene". APS News. Series II 18 (9): 2. 2009. http://www.aps.org/publications/apsnews/200910/loader.cfm?csModule=security/getfile&pageid=187967. Retrieved 6 October 2013.
12. ↑ "Discovery of graphene - Graphene - The University of Manchester". https://www.graphene.manchester.ac.uk/learn/discovery-of-graphene/.
13. ↑ "The Nobel Prize in Physics 2010". Nobel Foundation. https://www.nobelprize.org/prizes/physics/2010/summary/.
14. ↑ "Mass-Producing Graphene". 6 April 2018. https://www.americanscientist.org/article/mass-producing-graphene.
15. ↑ Joshi, Rita (8 April 2024). "Can Graphene Be Mass Produced?". https://www.azonano.com/article.aspx?ArticleID=6716.
16. ↑ "Global Demand for Graphene after Commercial Production to be Enormous, says Report". AZONANO.com. 28 February 2014. http://www.azonano.com/news.aspx?newsID=29510.
17. ↑ Mrmak, Nebojsa (28 November 2014). "Graphene properties (A Complete Reference)". http://www.graphene-battery.net/graphene-properties.htm.
18. ↑ "graphene layer". IUPAC Compendium of Chemical Terminology. International Union of Pure and Applied Chemistry. 2009. doi:10.1351/goldbook.G02683. ISBN 978-0-9678550-9-7. http://goldbook.iupac.org/G02683.html. Retrieved 31 March 2012.
19. ↑ 19.0 19.1 Geim, A. (2009). "Graphene: Status and Prospects". Science 324 (5934): 1530–4. doi:10.1126/science.1158877. PMID 19541989. Bibcode: 2009Sci...324.1530G.
20. ↑ Riedl, C.; Coletti, C.; Iwasaki, T.; Zakharov, A. A.; Starke, U. (2009). "Quasi-Free-Standing Epitaxial Graphene on SiC Obtained by Hydrogen Intercalation". Physical Review Letters 103 (24). doi:10.1103/PhysRevLett.103.246804. PMID 20366220. Bibcode: 2009PhRvL.103x6804R.
21. ↑ Geim, A. K. (2012). "Graphene Prehistory". Physica Scripta T146. doi:10.1088/0031-8949/2012/T146/014003. Bibcode: 2012PhST..146a4003G.
22. ↑ Brodie, B. C. (1859). "On the Atomic Weight of Graphite". Philosophical Transactions of the Royal Society of London 149 (149): 249–259. doi:10.1098/rstl.1859.0013. Bibcode: 1859RSPT..149..249B.
23. ↑ Debije, Peter; Scherrer, Paul (1916). "Interferenz an regellos orientierten Teilchen im Röntgenlicht I" (in de). Physikalische Zeitschrift 17: 277. http://resolver.sub.uni-goettingen.de/purl?PPN252457811_1916/dmdlog4. Retrieved 13 April 2014.
24. ↑ Debye, Peter; Scherrer, Paul (1917). "Über die Konstitution von Graphit und amorpher Kohle" (in de). Nachrichten von der Gesellschaft der Wissenschaften zu Göttingen, Mathematisch-Physikalische Klasse 1917: 180–188. https://eudml.org/doc/58985.
25. ↑ Hull, Albert W. (1917). "A New Method of X-ray Crystal Analysis". Phys. Rev. 10 (6): 661–696. doi:10.1103/PhysRev.10.661. Bibcode: 1917PhRv...10..661H.
26. ↑ Kohlschütter, V.; Haenni, P. (1919). "Zur Kenntnis des Graphitischen Kohlenstoffs und der Graphitsäure" (in de). Zeitschrift für anorganische und allgemeine Chemie 105 (1): 121–144. doi:10.1002/zaac.19191050109. Bibcode: 1919ZAACh.105..121K. https://zenodo.org/record/1428166. Retrieved 12 April 2020.
27. ↑ Bernal, John Desmond (1924). "The Structure of Graphite". Proc. R. Soc. Lond. A106 (740): 749–773. doi:10.1098/rspa.1924.0101. Bibcode: 1924RSPSA.106..749B.
28. ↑ Trucano, Peter; Chen, Ruey (13 November 1975). "Structure of graphite by neutron diffraction". Nature 258 (5531): 136–137. doi:10.1038/258136a0. Bibcode: 1975Natur.258..136T.
29. ↑ Howe, J. Y.; Rawn, C. J.; Jones, L. E.; Ow, H. (June 2003). "Improved crystallographic data for graphite". Powder Diffraction 18 (2): 150–154. doi:10.1154/1.1536926. Bibcode: 2003PDiff..18..150H.
30. ↑ 30.0 30.1 30.2 30.3 30.4 30.5 Semenoff, Gordon W. (24 December 1984). "Condensed-Matter Simulation of a Three-Dimensional Anomaly". Physical Review Letters 53 (26): 2449–2452. doi:10.1103/PhysRevLett.53.2449. Bibcode: 1984PhRvL..53.2449S.
31. ↑ DiVincenzo, D. P.; Mele, E. J. (1984). "Self-Consistent Effective Mass Theory for Intralayer Screening in Graphite Intercalation Compounds". Physical Review B 295 (4): 1685–1694. doi:10.1103/PhysRevB.29.1685. Bibcode: 1984PhRvB..29.1685D.
32. ↑ 32.0 32.1 32.2 32.3 32.4 32.5 Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; Katsnelson, M. I.; Grigorieva, I. V.; Dubonos, S. V.; Firsov, A. A. (2005). "Two-dimensional gas of massless Dirac fermions in graphene". Nature 438 (7065): 197–200. doi:10.1038/nature04233. PMID 16281030. Bibcode: 2005Natur.438..197N.
33. ↑ 33.0 33.1 Gusynin, V. P.; Sharapov, S. G. (2005). "Unconventional Integer Quantum Hall Effect in Graphene". Physical Review Letters 95 (14). doi:10.1103/PhysRevLett.95.146801. PMID 16241680. Bibcode: 2005PhRvL..95n6801G.
34. ↑ 34.0 34.1 34.2 Zhang, Y.; Tan, Y. W.; Stormer, H. L.; Kim, P. (2005). "Experimental observation of the quantum Hall effect and Berry's phase in graphene". Nature 438 (7065): 201–204. doi:10.1038/nature04235. PMID 16281031. Bibcode: 2005Natur.438..201Z.
35. ↑ Ruess, G.; Vogt, F. (1948). "Höchstlamellarer Kohlenstoff aus Graphitoxyhydroxyd" (in de). Monatshefte für Chemie 78 (3–4): 222–242. doi:10.1007/BF01141527.
36. ↑ 36.0 36.1 36.2 36.3 Meyer, J.; Geim, A. K.; Katsnelson, M. I.; Novoselov, K. S.; Booth, T. J.; Roth, S. (2007). "The structure of suspended graphene sheets". Nature 446 (7131): 60–63. doi:10.1038/nature05545. PMID 17330039. Bibcode: 2007Natur.446...60M.
37. ↑ 37.0 37.1 Harris, Peter (12 January 2018). "Transmission Electron Microscopy of Carbon: A Brief History". C 4 (1): 4. doi:10.3390/c4010004.
38. ↑ Boehm, H. P.; Clauss, A.; Fischer, G.; Hofmann, U. (1962). "Surface Properties of Extremely Thin Graphite Lamellae". Proceedings of the Fifth Conference on Carbon. Pergamon Press. http://www.americancarbonsociety.org/sites/default/files/conference/1961/1961_V1_73.PDF. Retrieved 1 April 2016.
39. ↑ van Bommel, A. J.; Crombeen, J. E.; van Tooren, A. (1975). "LEED and Auger electron observations of the SiC(0001) surface". Surface Science 48 (2): 463–472. doi:10.1016/0039-6028(75)90419-7. Bibcode: 1975SurSc..48..463V.
40. ↑ Oshima, C.; Nagashima, A. (1997). "Ultra-thin epitaxial films of graphite and hexagonal boron nitride on solid surfaces". J. Phys.: Condens. Matter 9 (1): 1–20. doi:10.1088/0953-8984/9/1/004. Bibcode: 1997JPCM....9....1O.
41. ↑ Forbeaux, I.; Themlin, J.-M.; Debever, J.-M. (1998). "Heteroepitaxial graphite on 6H-SiC(0001): Interface formation through conduction-band electronic structure". Physical Review B 58 (24): 16396–16406. doi:10.1103/PhysRevB.58.16396. Bibcode: 1998PhRvB..5816396F.
42. ↑ Boehm, H. P.; Setton, R.; Stumpp, E. (1986). "Nomenclature and terminology of graphite intercalation compounds". Carbon 24 (2): 241–245. doi:10.1016/0008-6223(86)90126-0. Bibcode: 1986Carbo..24..241B. "A single carbon layer of the graphitic structure would be the final member of infinite size of this series. The term graphene layer should be used for such a single carbon layer.".
43. ↑ Mouras, S. (1987). "Synthesis of first stage graphite intercalation compounds with fluorides". Revue de Chimie Minérale 24 (1): 572. doi:10.1016/0022-1139(87)95120-7. INIST:7578318. Bibcode: 1987JFluC..35..151H.
44. ↑ Saito, R.; Fujita, Mitsutaka; Dresselhaus, G.; Dresselhaus, M. (1992). "Electronic structure of graphene tubules based on C60". Physical Review B 46 (3): 1804–1811. doi:10.1103/PhysRevB.46.1804. PMID 10003828. Bibcode: 1992PhRvB..46.1804S.
45. ↑ Wang, S.; Yata, S.; Nagano, J.; Okano, Y.; Kinoshita, H.; Kikuta, H.; Yamabe, T. (2000). "A new carbonaceous material with large capacity and high efficiency for rechargeable Li-ion batteries". Journal of the Electrochemical Society 147 (7): 2498. doi:10.1149/1.1393559. Bibcode: 2000JElS..147.2498W.
46. ↑ Geim, A. K.; Kim, P. (April 2008). "Carbon Wonderland". Scientific American. https://www.scientificamerican.com/article.cfm?id=carbon-wonderland. ""... bits of graphene are undoubtedly present in every pencil mark""
47. ↑ Robert B. Rutherford and Richard L. Dudman (2002): "Ultra-thin flexible expanded graphite heating element ". US Patent 6667100. Filed on 2002-05-13, granted on 2003-12-23, assigned to EGC Operating Co LLC; expired.
48. ↑ Bor Z. Jang and Wen C. Huang (2002): "Nano-scaled graphene plates ". US Patent 7071258. Filed on 2002-10-21, granted on 2006-07-04, assigned to Global Graphene Group Inc; to expire on 6 January 2024.
49. ↑ "Graphene edges closer to widespread production and application". 10 August 2016. https://www.compositesworld.com/articles/cedar-ridge-research-receives-pioneer-patent-for-free-floating-graphene-production-technology.
50. ↑ 50.0 50.1 "The Story of Graphene". The University of Manchester. 10 September 2014. https://www.graphene.manchester.ac.uk/explore/the-story-of-graphene. ""Following discussions with colleagues, Andre and Kostya adopted a method that researchers in surface science were using – using simple Sellotape to peel away layers of graphite to expose a clean surface for study under the microscope.""
51. ↑ "Graphene pioneers bag Nobel prize". Institute of Physics, UK. 5 October 2010. http://physicsworld.com/cws/article/news/43939.
52. ↑ "The Nobel Prize in Physics 2010". The Nobel Foundation. https://www.nobelprize.org/prizes/physics/2010/illustrated-information/#reading.
53. ↑ "New £60m Engineering Innovation Centre to be based in Manchester". 10 September 2014. https://www.manchester.ac.uk/discover/news/new-60m-engineering-innovation-centre-to-be-based-in-manchester/.
54. ↑ Burn-Callander, Rebecca (1 July 2014). "Graphene maker aims to build British, billion-pound venture". Daily Telegraph. http://www.telegraph.co.uk/finance/businessclub/10936423/Graphene-maker-aims-to-build-British-billion-pound-venture.html.
55. ↑ Gibson, Robert (10 June 2014). "Consett firm Thomas Swan sees export success with grapheme". The Journal. http://www.thejournal.co.uk/business/business-news/consett-firm-thomas-swan-sees-7243084.
56. ↑ "Global breakthrough: Irish scientists discover how to mass produce 'wonder material' graphene". The Journal.ie. 20 April 2014. https://www.thejournal.ie/graphene-irish-researchers-major-breakdown-mass-production-1424843-Apr2014/.
57. ↑ "Cambridge Nanosystems opens new factory for commercial graphene production". Cambridge News. 16 June 2015. http://www.cambridge-news.co.uk/Cambridge-Nanosystems-opens-new-factory/story-26705678-detail/story.html.
58. ↑ Zdetsis, Aristides D.; Economou, E. N. (23 July 2015). "A Pedestrian Approach to the Aromaticity of Graphene and Nanographene: Significance of Huckel's (4 n +2)π Electron Rule". The Journal of Physical Chemistry C 119 (29): 16991–17003. doi:10.1021/acs.jpcc.5b04311.
59. ↑ Li, Zhilin; Chen, Lianlian; Meng, Sheng; Guo, Liwei; Huang, Jiao; Liu, Yu; Wang, Wenjun; Chen, Xiaolong (2015). "Field and temperature dependence of intrinsic diamagnetism in graphene: Theory and experiment". Phys. Rev. B 91 (9). doi:10.1103/PhysRevB.91.094429. Bibcode: 2015PhRvB..91i4429L.
60. ↑ 60.0 60.1 60.2 60.3 Cooper, Daniel R.; D'Anjou, Benjamin; Ghattamaneni, Nageswara; Harack, Benjamin; Hilke, Michael; Horth, Alexandre; Majlis, Norberto; Massicotte, Mathieu et al. (26 April 2012). "Experimental Review of Graphene". ISRN Condensed Matter Physics 2012: 1–56. doi:10.5402/2012/501686. Bibcode: 2011arXiv1110.6557C.
61. ↑ Félix, Isaac de Macêdo (2013). Estudo da estrutura eletrônica do grafeno e grafeno hidratado [Study of the electronic structure of graphene and hydrated graphene] (BS) (in português). Federal University of Campina Grande; National Council for Scientific and Technological Development.
62. ↑ Dixit, Vaibhav A.; Singh, Yashita Y. (June 2019). "How much aromatic are naphthalene and graphene?". Computational and Theoretical Chemistry 1162. doi:10.1016/j.comptc.2019.112504.
63. ↑ Delhaes, Pierre (21 December 2000). Graphite and Precursors. CRC Press. ISBN 978-90-5699-228-6. https://books.google.com/books?id=7p2pgNOWPbEC&q=sheet&pg=PA8.
64. ↑ Kasuya, D.; Yudasaka, M.; Takahashi, K.; Kokai, F.; Iijima, S. (2002). "Selective Production of Single-Wall Carbon Nanohorn Aggregates and Their Formation Mechanism". J. Phys. Chem. B 106 (19): 4947–4951. doi:10.1021/jp020387n. Bibcode: 2002JPCB..106.4947K.
65. ↑ Bernatowicz, T. J.; Gibbons, Patrick C.; Lodders, Katharina; Fegley, Bruce; Amari, Sachiko; Lewis, Roy S. (1996). "Constraints on stellar grain formation from presolar graphite in the Murchison meteorite". Astrophysical Journal 472 (2): 760–782. doi:10.1086/178105. Bibcode: 1996ApJ...472..760B.
66. ↑ Fraundorf, P.; Wackenhut, M. (2002). "The core structure of presolar graphite onions". Astrophysical Journal Letters 578 (2): L153–156. doi:10.1086/344633. Bibcode: 2002ApJ...578L.153F.
67. ↑ 67.0 67.1 Carlsson, J. M. (2007). "Graphene: Buckle or break". Nature Materials 6 (11): 801–2. doi:10.1038/nmat2051. PMID 17972931. Bibcode: 2007NatMa...6..801C.
68. ↑ 68.0 68.1 Fasolino, A.; Los, J. H.; Katsnelson, M. I. (2007). "Intrinsic ripples in graphene". Nature Materials 6 (11): 858–61. doi:10.1038/nmat2011. PMID 17891144. Bibcode: 2007NatMa...6..858F.
69. ↑ Meyer, Jannik C.; Geim, A. K.; Katsnelson, M. I.; Novoselov, K. S.; Booth, T. J.; Roth, S. (March 2007). "The structure of suspended graphene sheets". Nature 446 (7131): 60–63. doi:10.1038/nature05545. ISSN 1476-4687. PMID 17330039. Bibcode: 2007Natur.446...60M. https://www.nature.com/articles/nature05545.
70. ↑ 70.0 70.1 Ishigami, Masa (2007). "Atomic Structure of Graphene on SiO2". Nano Letters 7 (6): 1643–1648. doi:10.1021/nl070613a. PMID 17497819. Bibcode: 2007NanoL...7.1643I.
71. ↑ Shenderova, O. A.; Zhirnov, V. V.; Brenner, D. W. (July 2002). "Carbon Nanostructures". Critical Reviews in Solid State and Materials Sciences 27 (3–4): 227–356. doi:10.1080/10408430208500497. Bibcode: 2002CRSSM..27..227S.
72. ↑ 72.0 72.1 72.2 72.3 Neto, A Castro; Peres, N. M. R.; Novoselov, K. S.; Geim, A. K.; Geim, A. K. (2009). "The electronic properties of graphene". Rev Mod Phys 81 (1): 109–162. doi:10.1103/RevModPhys.81.109. Bibcode: 2009RvMP...81..109C. http://onnes.ph.man.ac.uk/nano/Publications/RMP_2009.pdf.
73. ↑ 73.0 73.1 73.2 73.3 Charlier, J.-C.; Eklund, P. C.; Zhu, J.; Ferrari, A. C. (2008). "Electron and Phonon Properties of Graphene: Their Relationship with Carbon Nanotubes". in Jorio, A.; Dresselhaus, G.; Dresselhaus, M. S.. Carbon Nanotubes: Advanced Topics in the Synthesis, Structure, Properties and Applications. Berlin/Heidelberg: Springer-Verlag. p. 673. https://books.google.com/books?id=ammoVEI-H2gC.
74. ↑ Kopelevich, Y.; Torres, J.; Da Silva, R.; Mrowka, F.; Kempa, H.; Esquinazi, P. (2003). "Reentrant Metallic Behavior of Graphite in the Quantum Limit". Physical Review Letters 90 (15). doi:10.1103/PhysRevLett.90.156402. PMID 12732058. Bibcode: 2003PhRvL..90o6402K.
75. ↑ Luk'yanchuk, Igor A.; Kopelevich, Yakov (2004). "Phase Analysis of Quantum Oscillations in Graphite". Physical Review Letters 93 (16). doi:10.1103/PhysRevLett.93.166402. PMID 15525015. Bibcode: 2004PhRvL..93p6402L.
76. ↑ Wallace, P. R. (1947). "The Band Theory of Graphite". Physical Review 71 (9): 622–634. doi:10.1103/PhysRev.71.622. Bibcode: 1947PhRv...71..622W.
77. ↑ 77.0 77.1 Avouris, P.; Chen, Z.; Perebeinos, V. (2007). "Carbon-based electronics". Nature Nanotechnology 2 (10): 605–15. doi:10.1038/nnano.2007.300. PMID 18654384. Bibcode: 2007NatNa...2..605A.
78. ↑ Lamas, C. A.; Cabra, D. C.; Grandi, N. (2009). "Generalized Pomeranchuk instabilities in graphene". Physical Review B 80 (7). doi:10.1103/PhysRevB.80.075108. Bibcode: 2009PhRvB..80g5108L.
79. ↑ Morozov, S. V.; Novoselov, K.; Katsnelson, M.; Schedin, F.; Elias, D.; Jaszczak, J.; Geim, A. (2008). "Giant Intrinsic Carrier Mobilities in Graphene and Its Bilayer". Physical Review Letters 100 (1). doi:10.1103/PhysRevLett.100.016602. PMID 18232798. Bibcode: 2008PhRvL.100a6602M.
80. ↑ 80.0 80.1 80.2 Chen, J. H.; Jang, Chaun; Xiao, Shudong; Ishigami, Masa; Fuhrer, Michael S. (2008). "Intrinsic and Extrinsic Performance Limits of Graphene Devices on SiO2". Nature Nanotechnology 3 (4): 206–9. doi:10.1038/nnano.2008.58. PMID 18654504.SiO2&rft.jtitle=Nature+Nanotechnology&rft.aulast=Chen&rft.aufirst=J.+H.&rft.au=Chen, J.+H.&rft.au=Jang, Chaun&rft.au=Xiao, Shudong&rft.au=Ishigami, Masa&rft.au=Fuhrer, Michael+S.&rft.date=2008&rft.volume=3&rft.issue=4&rft.pages=206–9&rft_id=info:doi/10.1038/nnano.2008.58&rft_id=info:pmid/18654504&rfr_id=info:sid/en.wikibooks.org:Physics:Graphene">
81. ↑ Akturk, A.; Goldsman, N. (2008). "Electron transport and full-band electron-phonon interactions in graphene". Journal of Applied Physics 103 (5): 053702–053702–8. doi:10.1063/1.2890147. Bibcode: 2008JAP...103e3702A.
82. ↑ "Physicists Show Electrons Can Travel More Than 100 Times Faster in Graphene". University Communications Newsdesk, University of Maryland . Newsdesk.umd.edu (24 March 2008). Retrieved on 12 January 2014.
83. ↑ Sagade, A. A. (2015). "Highly Air Stable Passivation of Graphene Based Field Effect Devices". Nanoscale 7 (8): 3558–3564. doi:10.1039/c4nr07457b. PMID 25631337. Bibcode: 2015Nanos...7.3558S.
84. ↑ "Graphene Devices Stand the Test of Time". 22 January 2015. https://spectrum.ieee.org/graphene-devices-stand-the-test-of-time.
85. ↑ "Researchers create superconducting graphene". Research & Development. 9 September 2015. http://www.rdmag.com/news/2015/09/researchers-create-superconducting-graphene.
86. ↑ 86.0 86.1 "New form of graphene allows electrons to behave like photons". kurzweilai.net. http://www.kurzweilai.net/new-form-of-graphene-allows-electrons-to-behave-like-photons.
87. ↑ Baringhaus, J.; Ruan, M.; Edler, F.; Tejeda, A.; Sicot, M.; Taleb-Ibrahimi, A.; Li, A. P.; Jiang, Z. et al. (2014). "Exceptional ballistic transport in epitaxial graphene nanoribbons". Nature 506 (7488): 349–354. doi:10.1038/nature12952. PMID 24499819. Bibcode: 2014Natur.506..349B.
88. ↑ 88.0 88.1 88.2 Chen, J. H.; Jang, C.; Adam, S.; Fuhrer, M. S.; Williams, E. D.; Ishigami, M. (2008). "Charged Impurity Scattering in Graphene". Nature Physics 4 (5): 377–381. doi:10.1038/nphys935. Bibcode: 2008NatPh...4..377C.
89. ↑ Light pulses control how graphene conducts electricity . kurzweilai.net. 4 August 2014
90. ↑ 90.0 90.1 Schedin, F.; Geim, A. K.; Morozov, S. V.; Hill, E. W.; Blake, P.; Katsnelson, M. I.; Novoselov, K. S. (2007). "Detection of individual gas molecules adsorbed on graphene". Nature Materials 6 (9): 652–655. doi:10.1038/nmat1967. PMID 17660825. Bibcode: 2007NatMa...6..652S.
91. ↑ Adam, S.; Hwang, E. H.; Galitski, V. M.; Das Sarma, S. (2007). "A self-consistent theory for graphene transport". Proc. Natl. Acad. Sci. USA 104 (47): 18392–7. doi:10.1073/pnas.0704772104. PMID 18003926. Bibcode: 2007PNAS..10418392A.
92. ↑ Steinberg, Hadar et al. (2008). "Charge fractionalization in quantum wires (Letter)". Nature Physics 4 (2): 116–119. doi:10.1038/nphys810. Bibcode: 2008NatPh...4..116S.
93. ↑ Trisetyarso, Agung (2012). "Dirac four-potential tunings-based quantum transistor utilizing the Lorentz force". Quantum Information & Computation 12 (11–12): 989. doi:10.26421/QIC12.11-12-7. Bibcode: 2010arXiv1003.4590T. http://dl.acm.org/citation.cfm?id=2481569.2481576. Retrieved 6 August 2013.
94. ↑ Pachos, Jiannis K. (2009). "Manifestations of topological effects in graphene". Contemporary Physics 50 (2): 375–389. doi:10.1080/00107510802650507. Bibcode: 2009ConPh..50..375P.
Franz, M. (5 January 2008). "Fractionalization of charge and statistics in graphene and related structures". University of British Columbia. http://www.int.washington.edu/talks/WorkShops/int_08_37W/People/Franz_M/Franz.pdf.
95. ↑ Peres, N. M. R. (15 September 2010). "Colloquium: The transport properties of graphene: An introduction". Reviews of Modern Physics 82 (3): 2673–2700. doi:10.1103/RevModPhys.82.2673. Bibcode: 2010RvMP...82.2673P.
96. ↑ Kim, Kuen Soo; Zhao, Yue; Jang, Houk; Lee, Sang Yoon; Kim, Jong Min; Kim, Kwang S.; Ahn, Jong-Hyun; Kim, Philip et al. (2009). "Large-scale pattern growth of graphene films for stretchable transparent electrodes". Nature 457 (7230): 706–10. doi:10.1038/nature07719. PMID 19145232. Bibcode: 2009Natur.457..706K.
97. ↑ 97.0 97.1 Jobst, Johannes; Waldmann, Daniel; Speck, Florian; Hirner, Roland; Maude, Duncan K.; Seyller, Thomas; Weber, Heiko B. (2009). "How Graphene-like is Epitaxial Graphene? Quantum Oscillations and Quantum Hall Effect". Physical Review B 81 (19). doi:10.1103/PhysRevB.81.195434. Bibcode: 2010PhRvB..81s5434J.
98. ↑ 98.0 98.1 Shen, T.; Gu, J. J.; Xu, M.; Wu, Y. Q.; Bolen, M. L.; Capano, M. A.; Engel, L. W.; Ye, P. D. (2009). "Observation of quantum-Hall effect in gated epitaxial graphene grown on SiC (0001)". Applied Physics Letters 95 (17): 172105. doi:10.1063/1.3254329. Bibcode: 2009ApPhL..95q2105S.
99. ↑ 99.0 99.1 Wu, Xiaosong; Hu, Yike; Ruan, Ming; Madiomanana, Nerasoa K.; Hankinson, John; Sprinkle, Mike; Berger, Claire; de Heer, Walt A. (2009). "Half integer quantum Hall effect in high mobility single layer epitaxial graphene". Applied Physics Letters 95 (22): 223108. doi:10.1063/1.3266524. Bibcode: 2009ApPhL..95v3108W.
100. ↑ 100.0 100.1 Lara-Avila, Samuel; Kalaboukhov, Alexei; Paolillo, Sara; Syväjärvi, Mikael; Yakimova, Rositza; Fal'ko, Vladimir; Tzalenchuk, Alexander; Kubatkin, Sergey (7 July 2009). "SiC Graphene Suitable For Quantum Hall Resistance Metrology". Science Brevia. Bibcode: 2009arXiv0909.1193L.
101. ↑ 101.0 101.1 Alexander-Webber, J. A.; Baker, A. M. R.; Janssen, T. J. B. M.; Tzalenchuk, A.; Lara-Avila, S.; Kubatkin, S.; Yakimova, R.; Piot, B. A. et al. (2013). "Phase Space for the Breakdown of the Quantum Hall Effect in Epitaxial Graphene". Physical Review Letters 111 (9). doi:10.1103/PhysRevLett.111.096601. PMID 24033057. Bibcode: 2013PhRvL.111i6601A.
102. ↑ Fuhrer, Michael S. (2009). "A physicist peels back the layers of excitement about graphene". Nature 459 (7250): 1037. doi:10.1038/4591037e. PMID 19553953. Bibcode: 2009Natur.459.1037F.
103. ↑ 103.0 103.1 103.2 Fuhrer, M. S. (2013). "Critical Mass in Graphene". Science 340 (6139): 1413–1414. doi:10.1126/science.1240317. PMID 23788788. Bibcode: 2013Sci...340.1413F.
104. ↑ 104.0 104.1 104.2 Yoon, Hosang; Forsythe, Carlos; Wang, Lei; Tombros, Nikolaos; Watanabe, Kenji; Taniguchi, Takashi; Hone, James; Kim, Philip et al. (2014). "Measurement of collective dynamical mass of Dirac fermions in graphene". Nature Electronics 9 (8): 594–599. doi:10.1038/nnano.2014.112. PMID 24952474. Bibcode: 2014NatNa...9..594Y.
105. ↑ 105.0 105.1 Zhang, Y.; Jiang, Z.; Small, J. P.; Purewal, M. S.; Tan, Y.-W.; Fazlollahi, M.; Chudow, J. D.; Jaszczak, J. A. et al. (2006). "Landau-Level Splitting in Graphene in High Magnetic Fields". Physical Review Letters 96 (13). doi:10.1103/PhysRevLett.96.136806. PMID 16712020. Bibcode: 2006PhRvL..96m6806Z.
106. ↑ 106.0 106.1 106.2 106.3 Du, X.; Skachko, Ivan; Duerr, Fabian; Luican, Adina; Andrei, Eva Y. (2009). "Fractional quantum Hall effect and insulating phase of Dirac electrons in graphene". Nature 462 (7270): 192–195. doi:10.1038/nature08522. PMID 19829294. Bibcode: 2009Natur.462..192D.
107. ↑ 107.0 107.1 Bolotin, K.; Ghahari, Fereshte; Shulman, Michael D.; Stormer, Horst L.; Kim, Philip (2009). "Observation of the fractional quantum Hall effect in graphene". Nature 462 (7270): 196–199. doi:10.1038/nature08582. PMID 19881489. Bibcode: 2009Natur.462..196B.
108. ↑ Bordag, M.; Fialkovsky, I. V.; Gitman, D. M.; Vassilevich, D. V. (2009). "Casimir interaction between a perfect conductor and graphene described by the Dirac model". Physical Review B 80 (24). doi:10.1103/PhysRevB.80.245406. Bibcode: 2009PhRvB..80x5406B.
109. ↑ Fialkovsky, I. V.; Marachevsky, V. N.; Vassilevich, D. V. (2011). "Finite temperature Casimir effect for graphene". Physical Review B 84 (3). doi:10.1103/PhysRevB.84.035446. Bibcode: 2011PhRvB..84c5446F.
110. ↑ Dobson, J. F.; White, A.; Rubio, A. (2006). "Asymptotics of the dispersion interaction: analytic benchmarks for van der Waals energy functionals". Physical Review Letters 96 (7). doi:10.1103/PhysRevLett.96.073201. PMID 16606085. Bibcode: 2006PhRvL..96g3201D.
111. ↑ Cismaru, Alina; Dragoman, Mircea; Dinescu, Adrian; Dragoman, Daniela; Stavrinidis, G.; Konstantinidis, G. (2013). "Microwave and Millimeter-wave Electrical Permittivity of Graphene Monolayer". arXiv:1309.0990 [cond-mat.mes-hall].
112. ↑ Kuzmenko, A. B.; Van Heumen, E.; Carbone, F.; Van Der Marel, D. (2008). "Universal infrared conductance of graphite". Physical Review Letters 100 (11). doi:10.1103/PhysRevLett.100.117401. PMID 18517825. Bibcode: 2008PhRvL.100k7401K.
113. ↑ "Graphene Gazing Gives Glimpse Of Foundations Of Universe". 4 April 2008. http://www.sciencedaily.com/releases/2008/04/080403140918.htm.
114. ↑ Jussila, Henri; Yang, He; Granqvist, Niko; Sun, Zhipei (5 February 2016). "Surface plasmon resonance for characterization of large-area atomic-layer graphene film". Optica 3 (2): 151–158. doi:10.1364/OPTICA.3.000151. Bibcode: 2016Optic...3..151J.
115. ↑ Lin, Xiao; Xu, Yang; Zhang, Baile; Hao, Ran; Chen, Hongsheng; Li, Erping (2013). "Unidirectional surface plasmons in nonreciprocal graphene". New Journal of Physics 15 (11). doi:10.1088/1367-2630/15/11/113003. Bibcode: 2013NJPh...15k3003L.
116. ↑ Zhang, Y.; Tang, Tsung-Ta; Girit, Caglar; Hao, Zhao; Martin, Michael C.; Zettl, Alex; Crommie, Michael F.; Shen, Y. Ron et al. (11 June 2009). "Direct observation of a widely tunable bandgap in bilayer graphene". Nature 459 (7248): 820–823. doi:10.1038/nature08105. PMID 19516337. Bibcode: 2009Natur.459..820Z.
117. ↑ Liu, Junfeng; Wright, A. R.; Zhang, Chao; Ma, Zhongshui (29 July 2008). "Strong terahertz conductance of graphene nanoribbons under a magnetic field". Appl Phys Lett 93 (4): 041106–041110. doi:10.1063/1.2964093. Bibcode: 2008ApPhL..93d1106L. https://ro.uow.edu.au/engpapers/3322. Retrieved 30 August 2019.
118. ↑ 118.0 118.1 Kurum, U.; Liu, Bo; Zhang, Kailiang; Liu, Yan; Zhang, Hao (2011). "Electrochemically tunable ultrafast optical response of graphene oxide". Applied Physics Letters 98 (2): 141103. doi:10.1063/1.3540647. Bibcode: 2011ApPhL..98b1103M.
119. ↑ Sreekanth, K. V.; Zeng, Shuwen; Shang, Jingzhi; Yong, Ken-Tye; Yu, Ting (2012). "Excitation of surface electromagnetic waves in a graphene-based Bragg grating". Scientific Reports 2. doi:10.1038/srep00737. PMID 23071901. Bibcode: 2012NatSR...2..737S.
120. ↑ Bao, Qiaoliang; Zhang, Han; Wang, Yu; Ni, Zhenhua; Yan, Yongli; Shen, Ze Xiang; Loh, Kian Ping; Tang, Ding Yuan (9 October 2009). "Atomic-Layer Graphene as a Saturable Absorber for Ultrafast Pulsed Lasers". Advanced Functional Materials 19 (19): 3077–3083. doi:10.1002/adfm.200901007. Bibcode: 2009AdvFM..19.3077B.
121. ↑ Zhang, H.; Tang, D. Y.; Zhao, L. M.; Bao, Q. L.; Loh, K. P. (28 September 2009). "Large energy mode locking of an erbium-doped fiber laser with atomic layer graphene". Optics Express 17 (20): 17630–17635. doi:10.1364/OE.17.017630. PMID 19907547. Bibcode: 2009OExpr..1717630Z.
122. ↑ Zhang, Han; Bao, Qiaoliang; Tang, Dingyuan; Zhao, Luming; Loh, Kianping (5 October 2009). "Large energy soliton erbium-doped fiber laser with a graphene-polymer composite mode locker". Applied Physics Letters 95 (14): 141103. doi:10.1063/1.3244206. Bibcode: 2009ApPhL..95n1103Z.
123. ↑ Zhang, Han; Tang, Dingyuan; Knize, R. J.; Zhao, Luming; Bao, Qiaoliang; Loh, Kian Ping (15 March 2010). "Graphene mode locked, wavelength-tunable, dissipative soliton fiber laser". Applied Physics Letters 96 (11): 111112. doi:10.1063/1.3367743. Bibcode: 2010ApPhL..96k1112Z.
124. ↑ Zhang (2009). "Graphene: Mode-locked lasers". NPG Asia Materials. doi:10.1038/asiamat.2009.52.
125. ↑ Zheng, Z.; Zhao, Chujun; Lu, Shunbin; Chen, Yu; Li, Ying; Zhang, Han; Wen, Shuangchun (2012). "Microwave and optical saturable absorption in graphene". Optics Express 20 (21): 23201–23214. doi:10.1364/OE.20.023201. PMID 23188285. Bibcode: 2012OExpr..2023201Z.
126. ↑ Zhang, H.; Virally, Stéphane; Bao, Qiaoliang; Kian Ping, Loh; Massar, Serge; Godbout, Nicolas; Kockaert, Pascal (2012). "Z-scan measurement of the nonlinear refractive index of graphene". Optics Letters 37 (11): 1856–1858. doi:10.1364/OL.37.001856. PMID 22660052. Bibcode: 2012OptL...37.1856Z.
127. ↑ Dong, H.; Conti, C.; Marini, A.; Biancalana, F. (2013). "Terahertz relativistic spatial solitons in doped graphene metamaterials". Journal of Physics B: Atomic, Molecular and Optical Physics 46 (15): 15540. doi:10.1088/0953-4075/46/15/155401. Bibcode: 2013JPhB...46o5401D.
128. ↑ Onida, Giovanni; Rubio, Angel (2002). "Electronic excitations: Density-functional versus many-body Green's-function approaches". Rev. Mod. Phys. 74 (2): 601–659. doi:10.1103/RevModPhys.74.601. Bibcode: 2002RvMP...74..601O. https://digital.csic.es/bitstream/10261/98472/1/Electronic excitations.pdf. Retrieved 23 September 2019.
129. ↑ Yang, Li; Deslippe, Jack; Park, Cheol-Hwan; Cohen, Marvin; Louie, Steven (2009). "Excitonic Effects on the Optical Response of Graphene and Bilayer Graphene". Physical Review Letters 103 (18). doi:10.1103/PhysRevLett.103.186802. PMID 19905823. Bibcode: 2009PhRvL.103r6802Y.
130. ↑ Prezzi, Deborah; Varsano, Daniele; Ruini, Alice; Marini, Andrea; Molinari, Elisa (2008). "Optical properties of graphene nanoribbons: The role of many-body effects". Physical Review B 77 (4). doi:10.1103/PhysRevB.77.041404. Bibcode: 2008PhRvB..77d1404P.
Yang, Li; Cohen, Marvin L.; Louie, Steven G. (2007). "Excitonic Effects in the Optical Spectra of Graphene Nanoribbons". Nano Letters 7 (10): 3112–5. doi:10.1021/nl0716404. PMID 17824720. Bibcode: 2007NanoL...7.3112Y.
Yang, Li; Cohen, Marvin L.; Louie, Steven G. (2008). "Magnetic Edge-State Excitons in Zigzag Graphene Nanoribbons". Physical Review Letters 101 (18). doi:10.1103/PhysRevLett.101.186401. PMID 18999843. Bibcode: 2008PhRvL.101r6401Y.
131. ↑ Zhu, Xi; Su, Haibin (2010). "Excitons of Edge and Surface Functionalized Graphene Nanoribbons". J. Phys. Chem. C 114 (41): 17257–17262. doi:10.1021/jp102341b. https://figshare.com/articles/Excitons_of_Edge_and_Surface_Functionalized_Graphene_Nanoribbons/2719792. Retrieved 1 December 2019.
132. ↑ Wang, Min; Li, Chang Ming (2011). "Excitonic properties of hydrogen saturation-edged armchair graphene nanoribbons". Nanoscale 3 (5): 2324–8. doi:10.1039/c1nr10095e. PMID 21503364. Bibcode: 2011Nanos...3.2324W.
133. ↑ Bolmatov, Dima; Mou, Chung-Yu (2010). "Josephson effect in graphene SNS junction with a single localized defect". Physica B 405 (13): 2896–2899. doi:10.1016/j.physb.2010.04.015. Bibcode: 2010PhyB..405.2896B.
Bolmatov, Dima; Mou, Chung-Yu (2010). "Tunneling conductance of the graphene SNS junction with a single localized defect". Journal of Experimental and Theoretical Physics 110 (4): 613–617. doi:10.1134/S1063776110040084. Bibcode: 2010JETP..110..613B.
134. ↑ Zhu, Xi; Su, Haibin (2011). "Scaling of Excitons in Graphene Nanoribbons with Armchair Shaped Edges". Journal of Physical Chemistry A 115 (43): 11998–12003. doi:10.1021/jp202787h. PMID 21939213. Bibcode: 2011JPCA..11511998Z. https://figshare.com/articles/Scaling_of_Excitons_in_Graphene_Nanoribbons_with_Armchair_Shaped_Edges/2590648. Retrieved 1 December 2019.
135. ↑ 135.0 135.1 Tombros, Nikolaos (2007). "Electronic spin transport and spin precession in single graphene layers at room temperature". Nature 448 (7153): 571–575. doi:10.1038/nature06037. PMID 17632544. Bibcode: 2007Natur.448..571T.
136. ↑ 136.0 136.1 Cho, Sungjae; Chen, Yung-Fu; Fuhrer, Michael S. (2007). "Gate-tunable Graphene Spin Valve". Applied Physics Letters 91 (12): 123105. doi:10.1063/1.2784934. Bibcode: 2007ApPhL..91l3105C.
137. ↑ Ohishi, Megumi (2007). "Spin Injection into a Graphene Thin Film at Room Temperature". Jpn J Appl Phys 46 (25): L605–L607. doi:10.1143/JJAP.46.L605. Bibcode: 2007JaJAP..46L.605O.
138. ↑ Hashimoto, T.; Kamikawa, S.; Yagi, Y.; Haruyama, J.; Yang, H.; Chshiev, M. (2014). "Graphene edge spins: spintronics and magnetism in graphene nanomeshes". Nanosystems: Physics, Chemistry, Mathematics 5 (1): 25–38. http://nanojournal.ifmo.ru/en/wp-content/uploads/2014/02/NPCM51_P25-38.pdf. Retrieved 2 May 2019.
139. ↑ Xin, Na; Lourembam, James; Kumaravadivel, Piranavan (April 2023). "Giant magnetoresistance of Dirac plasma in high-mobility graphene". Nature 616 (7956): 270–274. doi:10.1038/s41586-023-05807-0. PMID 37045919. Bibcode: 2023Natur.616..270X.
140. ↑ Weser, M.; Rehder, Y.; Horn, K.; Sicot, M.; Fonin, M.; Preobrajenski, A. B.; Voloshina, E. N.; Goering, E.; Dedkov, Yu. S. "Induced magnetism of carbon atoms at the graphene/Ni(111) interface".
141. ↑ Hashimoto, T.; Kamikawa, S.; Yagi, Y.; Haruyama, J.; Yang, H.; Chshiev, M. "Graphene edge spins: spintronics and magnetism in graphene nanomeshes" , February 2014, Volume 5, Issue 1, pp. 25.
142. ↑ Coxworth, Ben (27 January 2015). "Scientists give graphene one more quality – magnetism". Gizmag. http://www.gizmag.com/magnetized-graphene/35805.
143. ↑ Class for Physics of the Royal Swedish Academy of Sciences (5 October 2010). "Scientific Background on the Nobel Prize in Physics 2010 GRAPHENE". Nobel Prize. http://www.nobelprize.org/nobel_prizes/physics/laureates/2010/advanced-physicsprize2010.pdf.
144. ↑ Briggs, Benjamin D.; Nagabhirava, Bhaskar; Rao, Gayathri; Deer, Robert; Gao, Haiyuan; Xu, Yang; Yu, Bin (2010). "Electromechanical robustness of monolayer graphene with extreme bending". Applied Physics Letters 97 (22): 223102. doi:10.1063/1.3519982. Bibcode: 2010ApPhL..97v3102B.
145. ↑ Frank, I. W.; Tanenbaum, D. M.; Van Der Zande, A. M.; McEuen, P. L. (2007). "Mechanical properties of suspended graphene sheets". Journal of Vacuum Science & Technology B: Microelectronics and Nanometer Structures 25 (6): 2558–2561. doi:10.1116/1.2789446. Bibcode: 2007JVSTB..25.2558F. https://www.lassp.cornell.edu/lassp_data/mceuen/homepage/Publications/JVSTB_Pushing_Graphene.pdf. Retrieved 21 April 2009.
146. ↑ Braga, S.; Coluci, V. R.; Legoas, S. B.; Giro, R.; Galvão, D. S.; Baughman, R. H. (2004). "Structure and Dynamics of Carbon Nanoscrolls". Nano Letters 4 (5): 881–884. doi:10.1021/nl0497272. Bibcode: 2004NanoL...4..881B.
147. ↑ Bolmatov, Dima; Mou, Chung-Yu (2011). "Graphene-based modulation-doped superlattice structures". Journal of Experimental and Theoretical Physics 112 (1): 102–107. doi:10.1134/S1063776111010043. Bibcode: 2011JETP..112..102B.
148. ↑ Bolmatov, Dima (2011). "Thermodynamic properties of tunneling quasiparticles in graphene-based structures". Physica C 471 (23–24): 1651–1654. doi:10.1016/j.physc.2011.07.008. Bibcode: 2011PhyC..471.1651B.
149. ↑ Grima, J. N.; Winczewski, S.; Mizzi, L.; Grech, M. C.; Cauchi, R.; Gatt, R.; Attard, D.; Wojciechowski, K. W. et al. (2014). "Tailoring Graphene to Achieve Negative Poisson's Ratio Properties". Advanced Materials 27 (8): 1455–1459. doi:10.1002/adma.201404106. PMID 25504060.
150. ↑ Ren, Zhaodi; Meng, Nan; Shehzad, Khurram; Xu, Yang; Qu, Shaoxing; Yu, Bin; Luo, Jack (2015). "Mechanical properties of nickel-graphene composites synthesized by electrochemical deposition". Nanotechnology 26 (6). doi:10.1088/0957-4484/26/6/065706. PMID 25605375. Bibcode: 2015Nanot..26f5706R. http://ubir.bolton.ac.uk/1575/1/Mechanical properties of nickel-graphene composites synthesized by electrochemical deposition.pdf. Retrieved 7 January 2020.
151. ↑ Zhang, Peng; Ma, Lulu; Fan, Feifei; Zeng, Zhi; Peng, Cheng; Loya, Phillip E.; Liu, Zheng; Gong, Yongji et al. (2014). "Fracture toughness of graphene". Nature Communications 5. doi:10.1038/ncomms4782. PMID 24777167. Bibcode: 2014NatCo...5.3782Z.
152. ↑ Dorrieron, Jason (4 December 2014). "Graphene Armor Would Be Light, Flexible and Far Stronger Than Steel". Singularity Hub. http://singularityhub.com/2014/12/04/graphene-armor-would-be-light-flexible-and-far-stronger-than-steel/.
153. ↑ Coxworth, Ben (1 December 2014). "Graphene could find use in lightweight ballistic body armor". Gizmag. http://www.gizmag.com/graphene-bulletproof-armor/35004.
154. ↑ Papageorgiou, Dimitrios G.; Kinloch, Ian A.; Young, Robert J. (October 2017). "Mechanical properties of graphene and graphene-based nanocomposites". Progress in Materials Science 90: 75–127. doi:10.1016/j.pmatsci.2017.07.004.
155. ↑ Li, J. C. M. (June 1972). "Disclination model of high angle grain boundaries". Surface Science 31: 12–26. doi:10.1016/0039-6028(72)90251-8. Bibcode: 1972SurSc..31...12L.
156. ↑ Grantab, R.; Shenoy, V. B.; Ruoff, R. S. (12 November 2010). "Anomalous Strength Characteristics of Tilt Grain Boundaries in Graphene". Science 330 (6006): 946–948. doi:10.1126/science.1196893. PMID 21071664. Bibcode: 2010Sci...330..946G.
157. ↑ Wei, Yujie; Wu, Jiangtao; Yin, Hanqing; Shi, Xinghua; Yang, Ronggui; Dresselhaus, Mildred (September 2012). "The nature of strength enhancement and weakening by pentagon–heptagon defects in graphene". Nature Materials 11 (9): 759–763. doi:10.1038/nmat3370. PMID 22751178. Bibcode: 2012NatMa..11..759W. http://dspace.imech.ac.cn/handle/311007/46051. Retrieved 30 August 2019.
158. ↑ Lee, G.-H.; Cooper, R. C.; An, S. J.; Lee, S.; van der Zande, A.; Petrone, N.; Hammerberg, A. G.; Lee, C. et al. (31 May 2013). "High-Strength Chemical-Vapor-Deposited Graphene and Grain Boundaries". Science 340 (6136): 1073–1076. doi:10.1126/science.1235126. PMID 23723231. Bibcode: 2013Sci...340.1073L.
159. ↑ Rasool, Haider I.; Ophus, Colin; Klug, William S.; Zettl, A.; Gimzewski, James K. (December 2013). "Measurement of the intrinsic strength of crystalline and polycrystalline graphene". Nature Communications 4 (1): 2811. doi:10.1038/ncomms3811. Bibcode: 2013NatCo...4.2811R.
160. ↑ 160.0 160.1 Zhang, Teng; Li, Xiaoyan; Gao, Huajian (November 2015). "Fracture of graphene: a review". International Journal of Fracture 196 (1–2): 1–31. doi:10.1007/s10704-015-0039-9. Bibcode: 2015IJFr..196....1Z.
161. ↑ Akinwande, Deji; Brennan, Christopher J.; Bunch, J. Scott; Egberts, Philip; Felts, Jonathan R.; Gao, Huajian; Huang, Rui; Kim, Joon-Seok et al. (May 2017). "A review on mechanics and mechanical properties of 2D materials—Graphene and beyond". Extreme Mechanics Letters 13: 42–77. doi:10.1016/j.eml.2017.01.008. Bibcode: 2017ExML...13...42A.
162. ↑ 162.0 162.1 Isacsson, Andreas; Cummings, Aron W.; Colombo, Luciano; Colombo, Luigi; Kinaret, Jari M.; Roche, Stephan (19 December 2016). "Scaling properties of polycrystalline graphene: A review". 2D Materials 4 (1): 012002. doi:10.1088/2053-1583/aa5147.
163. ↑ 163.0 163.1 Kotakoski, Jani; Meyer, Jannik C. (24 May 2012). "Mechanical properties of polycrystalline graphene based on a realistic atomistic model". Physical Review B 85 (19). doi:10.1103/PhysRevB.85.195447. Bibcode: 2012PhRvB..85s5447K.
164. ↑ 164.0 164.1 Song, Zhigong; Artyukhov, Vasilii I.; Yakobson, Boris I.; Xu, Zhiping (10 April 2013). "Pseudo Hall–Petch Strength Reduction in Polycrystalline Graphene". Nano Letters 13 (4): 1829–1833. doi:10.1021/nl400542n. PMID 23528068. Bibcode: 2013NanoL..13.1829S.
165. ↑ 165.0 165.1 Sha, Z. D.; Quek, S. S.; Pei, Q. X.; Liu, Z. S.; Wang, T. J.; Shenoy, V. B.; Zhang, Y. W. (May 2015). "Inverse Pseudo Hall-Petch Relation in Polycrystalline Graphene". Scientific Reports 4 (1): 5991. doi:10.1038/srep05991. PMID 25103818. Bibcode: 2014NatSR...4.5991S.
166. ↑ Berber, Savas; Kwon, Young-Kyun; Tománek, David (2000). "Unusually High Thermal Conductivity of Carbon Nanotubes". Phys. Rev. Lett. 84 (20): 4613–6. doi:10.1103/PhysRevLett.84.4613. PMID 10990753. Bibcode: 2000PhRvL..84.4613B.
167. ↑ 167.0 167.1 Balandin, A. A.; Ghosh, Suchismita; Bao, Wenzhong; Calizo, Irene; Teweldebrhan, Desalegne; Miao, Feng; Lau, Chun Ning (20 February 2008). "Superior Thermal Conductivity of Single-Layer Graphene". Nano Letters 8 (3): 902–907. doi:10.1021/nl0731872. PMID 18284217. Bibcode: 2008NanoL...8..902B.
168. ↑ Touloukian, Y. S. (1970). Thermophysical Properties of Matter: Thermal conductivity: nonmetallic solids. IFI/Plenum. ISBN 978-0-306-67020-6. https://books.google.com/books?id=31sqAAAAYAAJ.
169. ↑ Cai, Weiwei; Moore, Arden L.; Zhu, Yanwu; Li, Xuesong; Chen, Shanshan; Shi, Li; Ruoff, Rodney S. (2010). "Thermal Transport in Suspended and Supported Monolayer Graphene Grown by Chemical Vapor Deposition". Nano Letters 10 (5): 1645–1651. doi:10.1021/nl9041966. PMID 20405895. Bibcode: 2010NanoL..10.1645C.
170. ↑ Faugeras, Clement; Faugeras, Blaise; Orlita, Milan; Potemski, M.; Nair, Rahul R.; Geim, A. K. (2010). "Thermal Conductivity of Graphene in Corbino Membrane Geometry". ACS Nano 4 (4): 1889–1892. doi:10.1021/nn9016229. PMID 20218666. Bibcode: 2010ACSNa...4.1889F.
171. ↑ Xu, Xiangfan; Pereira, Luiz F. C.; Wang, Yu; Wu, Jing; Zhang, Kaiwen; Zhao, Xiangming; Bae, Sukang; Tinh Bui, Cong et al. (2014). "Length-dependent thermal conductivity in suspended single-layer graphene". Nature Communications 5. doi:10.1038/ncomms4689. PMID 24736666. Bibcode: 2014NatCo...5.3689X.
172. ↑ Lee, Jae-Ung; Yoon, Duhee; Kim, Hakseong; Lee, Sang Wook; Cheong, Hyeonsik (2011). "Thermal conductivity of suspended pristine graphene measured by Raman spectroscopy". Physical Review B 83 (8). doi:10.1103/PhysRevB.83.081419. Bibcode: 2011PhRvB..83h1419L.
173. ↑ Seol, J. H.; Jo, I.; Moore, A. L.; Lindsay, L.; Aitken, Z. H.; Pettes, M. T.; Li, X.; Yao, Z. et al. (2010). "Two-Dimensional Phonon Transport in Supported Graphene". Science 328 (5975): 213–216. doi:10.1126/science.1184014. PMID 20378814. Bibcode: 2010Sci...328..213S. https://hal-cea.archives-ouvertes.fr/cea-00818281. Retrieved 28 January 2023.
174. ↑ Klemens, P. G. (2001). "Theory of Thermal Conduction in Thin Ceramic Films". International Journal of Thermophysics 22 (1): 265–275. doi:10.1023/A:1006776107140.
175. ↑ Jang, Wanyoung; Chen, Zhen; Bao, Wenzhong; Lau, Chun Ning; Dames, Chris (2010). "Thickness-Dependent Thermal Conductivity of Encased Graphene and Ultrathin Graphite". Nano Letters 10 (10): 3909–3913. doi:10.1021/nl101613u. PMID 20836537. Bibcode: 2010NanoL..10.3909J.
176. ↑ Pettes, Michael Thompson; Jo, Insun; Yao, Zhen; Shi, Li (2011). "Influence of Polymeric Residue on the Thermal Conductivity of Suspended Bilayer Graphene". Nano Letters 11 (3): 1195–1200. doi:10.1021/nl104156y. PMID 21314164. Bibcode: 2011NanoL..11.1195P.
177. ↑ Chen, Shanshan; Wu, Qingzhi; Mishra, Columbia; Kang, Junyong; Zhang, Hengji; Cho, Kyeongjae; Cai, Weiwei; Balandin, Alexander A. et al. (2012). "Thermal conductivity of isotopically modified graphene". Nature Materials 11 (3): 203–207. 10 January 2012. doi:10.1038/nmat3207. PMID 22231598. Bibcode: 2012NatMa..11..203C.
Lay summary: Tracy, Suzanne (12 January 2012). "Keeping Electronics Cool". Scientific Computing (Advantage Business Media): scientificcomputing.com. http://www.scientificcomputing.com/news-HPC-Keeping-Electronics-Cool-011212.aspx?et_cid=2422972&et_rid=220285420&linkid=http://www.scientificcomputing.com/news-HPC-Keeping-Electronics-Cool-011212.aspx.
178. ↑ Saito, K.; Nakamura, J.; Natori, A. (2007). "Ballistic thermal conductance of a graphene sheet". Physical Review B 76 (11). doi:10.1103/PhysRevB.76.115409. Bibcode: 2007PhRvB..76k5409S.
179. ↑ Liang, Qizhen; Yao, Xuxia; Wang, Wei; Liu, Yan; Wong, Ching Ping (2011). "A Three-Dimensional Vertically Aligned Functionalized Multilayer Graphene Architecture: An Approach for Graphene-Based Thermal Interfacial Materials". ACS Nano 5 (3): 2392–2401. doi:10.1021/nn200181e. PMID 21384860. Bibcode: 2011ACSNa...5.2392L. https://figshare.com/articles/A_Three_Dimensional_Vertically_Aligned_Functionalized_Multilayer_Graphene_Architecture_An_Approach_for_Graphene_Based_Thermal_Interfacial_Materials/2680561. Retrieved 1 December 2019.
180. ↑ Delhaes, P. (2001). Graphite and Precursors. CRC Press. ISBN 978-90-5699-228-6. https://books.google.com/books?id=7p2pgNOWPbEC.
181. ↑ 181.0 181.1 Mingo, N.; Broido, D. A. (2005). "Carbon Nanotube Ballistic Thermal Conductance and Its Limits". Physical Review Letters 95 (9). doi:10.1103/PhysRevLett.95.096105. PMID 16197233. Bibcode: 2005PhRvL..95i6105M.
182. ↑ Mounet, N.; Marzari, N. (2005). "First-principles determination of the structural, vibrational and thermodynamic properties of diamond, graphite, and derivatives". Physical Review B 71 (20). doi:10.1103/PhysRevB.71.205214. Bibcode: 2005PhRvB..71t5214M.
183. ↑ Lifshitz, I. M. (1952) (in ru). Journal of Experimental and Theoretical Physics. 22. p. 475.
184. ↑ Bonaccorso, F.; Colombo, L.; Yu, G.; Stoller, M.; Tozzini, V.; Ferrari, A. C.; Ruoff, R. S.; Pellegrini, V. (2015). "Graphene, related two-dimensional crystals, and hybrid systems for energy conversion and storage". Science 347 (6217). doi:10.1126/science.1246501. PMID 25554791. Bibcode: 2015Sci...347...41B.
185. ↑ Denis, P. A.; Iribarne, F. (2013). "Comparative Study of Defect Reactivity in Graphene". Journal of Physical Chemistry C 117 (37): 19048–19055. doi:10.1021/jp4061945.
186. ↑ Yamada, Y. et al. (2014). "Subnanometer vacancy defects introduced on graphene by oxygen gas". Journal of the American Chemical Society 136 (6): 2232–2235. doi:10.1021/ja4117268. PMID 24460150. Bibcode: 2014JAChS.136.2232Y.
187. ↑ Eftekhari, A.; Jafarkhani, P. (2013). "Curly Graphene with Specious Interlayers Displaying Superior Capacity for Hydrogen Storage". Journal of Physical Chemistry C 117 (48): 25845–25851. doi:10.1021/jp410044v.
188. ↑ Yamada, Y.; Yasuda, H.; Murota, K.; Nakamura, M.; Sodesawa, T.; Sato, S. (2013). "Analysis of heat-treated graphite oxide by X-ray photoelectron spectroscopy". Journal of Materials Science 48 (23): 8171–8198. doi:10.1007/s10853-013-7630-0. Bibcode: 2013JMatS..48.8171Y.
189. ↑ Yamada, Y.; Kim, J.; Murota, K.; Matsuo, S.; Sato, S. (2014). "Nitrogen-containing graphene analyzed by X-ray photoelectron spectroscopy". Carbon 70: 59–74. doi:10.1016/j.carbon.2013.12.061. Bibcode: 2014Carbo..70...59Y.
190. ↑ "Thinnest graphene sheets react strongly with hydrogen atoms; thicker sheets are relatively unaffected". Phys.org. 1 February 2013. http://phys.org/news/2013-02-thinnest-graphene-sheets-react-strongly.html.
191. ↑ Zan, Recep; Ramasse, Quentin M.; Bangert, Ursel; Novoselov, Konstantin S. (2012). "Graphene Reknits Its Holes". Nano Letters 12 (8): 3936–3940. doi:10.1021/nl300985q. PMID 22765872. Bibcode: 2012NanoL..12.3936Z.
192. ↑ Bonaccorso, Francesco; Colombo, Luigi; Yu, Guihua; Stoller, Meryl; Tozzini, Valentina; Ferrari, Andrea C.; Ruoff, Rodney S.; Pellegrini, Vittorio (2 January 2015). "Graphene, related two-dimensional crystals, and hybrid systems for energy conversion and storage". Science 347 (6217). doi:10.1126/science.1246501. PMID 25554791. Bibcode: 2015Sci...347...41B.
193. ↑ Bullock, Christopher J.; Bussy, Cyrill (18 April 2019). "Biocompatibility Considerations in the Design of Graphene Biomedical Materials". Advanced Materials Interfaces 6 (11). doi:10.1002/admi.201900229.
194. ↑ Liao, Ken-Hsuan; Lin, Yu-Shen; Macosko, Christopher W.; Haynes, Christy L. (27 July 2011). "Cytotoxicity of Graphene Oxide and Graphene in Human Erythrocytes and Skin Fibroblasts". ACS Applied Materials & Interfaces 3 (7): 2607–2615. doi:10.1021/am200428v. PMID 21650218. Bibcode: 2011AAMI....3.2607L.
195. ↑ Fabbro, Alessandra; Scaini, Denis; León, Verónica; Vázquez, Ester; Cellot, Giada; Privitera, Giulia; Lombardi, Lucia; Torrisi, Felice et al. (26 January 2016). "Graphene-Based Interfaces Do Not Alter Target Nerve Cells". ACS Nano 10 (1): 615–623. doi:10.1021/acsnano.5b05647. PMID 26700626. Bibcode: 2016ACSNa..10..615F.
196. ↑ "Graphene shown to safely interact with neurons in the brain". 29 January 2016. https://www.cam.ac.uk/research/news/graphene-shown-to-safely-interact-with-neurons-in-the-brain.
197. ↑ Nayak, Tapas R.; Andersen, Henrik; Makam, Venkata S.; Khaw, Clement; Bae, Sukang; Xu, Xiangfan; Ee, Pui-Lai R.; Ahn, Jong-Hyun et al. (28 June 2011). "Graphene for Controlled and Accelerated Osteogenic Differentiation of Human Mesenchymal Stem Cells". ACS Nano 5 (6): 4670–4678. doi:10.1021/nn200500h. PMID 21528849. Bibcode: 2011ACSNa...5.4670N.
198. ↑ Tehrani, Z. (1 September 2014). "Generic epitaxial graphene biosensors for ultrasensitive detection of cancer risk biomarker". 2D Materials 1 (2). doi:10.1088/2053-1583/1/2/025004. Bibcode: 2014TDM.....1b5004T. https://cronfa.swan.ac.uk/Record/cronfa19735/Download/0019735-07052015130054.pdf. Retrieved 7 January 2020.
199. ↑ Xu, Yang; He, K. T.; Schmucker, S. W.; Guo, Z.; Koepke, J. C.; Wood, J. D.; Lyding, J. W.; Aluru, N. R. (2011). "Inducing Electronic Changes in Graphene through Silicon (100) Substrate Modification". Nano Letters 11 (7): 2735–2742. doi:10.1021/nl201022t. PMID 21661740. Bibcode: 2011NanoL..11.2735X.
200. ↑ Kula, Piotr; Pietrasik, Robert; Dybowski, Konrad; Atraszkiewicz, Radomir; Szymanski, Witold; Kolodziejczyk, Lukasz; Niedzielski, Piotr; Nowak, Dorota (2014). "Single and Multilayer Growth of Graphene from the Liquid Phase". Applied Mechanics and Materials 510: 8–12. doi:10.4028/www.scientific.net/AMM.510.8.
201. ↑ "Polish scientists find way to make super-strong graphene sheets | Graphene-Info". http://www.graphene-info.com/polish-scientists-find-way-make-super-strong-graphene-sheets.
202. ↑ Montenegro, Angelo; Dutta, Chayan; Mammetkuliev, Muhammet; Shi, Haotian; Hou, Bingya; Bhattacharyya, Dhritiman; Zhao, Bofan; Cronin, Stephen B. et al. (3 June 2021). "Asymmetric response of interfacial water to applied electric fields". Nature 594 (7861): 62–65. doi:10.1038/s41586-021-03504-4. PMID 34079138. Bibcode: 2021Natur.594...62M.
203. ↑ Min, Hongki; Sahu, Bhagawan; Banerjee, Sanjay; MacDonald, A. (2007). "Ab initio theory of gate induced gaps in graphene bilayers". Physical Review B 75 (15). doi:10.1103/PhysRevB.75.155115. Bibcode: 2007PhRvB..75o5115M.
204. ↑ Barlas, Yafis; Côté, R.; Lambert, J.; MacDonald, A. H. (2010). "Anomalous Exciton Condensation in Graphene Bilayers". Physical Review Letters 104 (9). doi:10.1103/PhysRevLett.104.096802. PMID 20367001. Bibcode: 2010PhRvL.104i6802B.
205. ↑ 205.0 205.1 Min, Lola; Hovden, Robert; Huang, Pinshane; Wojcik, Michal; Muller, David A.; Park, Jiwoong (2012). "Twinning and Twisting of Tri- and Bilayer Graphene". Nano Letters 12 (3): 1609–1615. doi:10.1021/nl204547v. PMID 22329410. Bibcode: 2012NanoL..12.1609B.
206. ↑ Forestier, Alexis; Balima, Félix; Bousige, Colin; de Sousa Pinheiro, Gardênia; Fulcrand, Rémy; Kalbác, Martin; San-Miguel, Alfonso (28 April 2020). "Strain and Piezo-Doping Mismatch between Graphene Layers". J. Phys. Chem. C 124 (20): 11193. doi:10.1021/acs.jpcc.0c01898. https://hal.archives-ouvertes.fr/hal-02651267/document. Retrieved 21 December 2020.
207. ↑ 207.0 207.1 Lenski, Daniel R.; Fuhrer, Michael S. (2011). "Raman and optical characterization of multilayer turbostratic graphene grown via chemical vapor deposition". Journal of Applied Physics 110 (1): 013720–013720–4. doi:10.1063/1.3605545. Bibcode: 2011JAP...110a3720L.
208. ↑ 208.0 208.1 Luong, Duy X.; Bets, Ksenia V.; Algozeeb, Wala Ali; Stanford, Michael G.; Kittrell, Carter; Chen, Weiyin; Salvatierra, Rodrigo V.; Ren, Muqing et al. (January 2020). "Gram-scale bottom-up flash graphene synthesis". Nature 577 (7792): 647–651. doi:10.1038/s41586-020-1938-0. ISSN 1476-4687. PMID 31988511. Bibcode: 2020Natur.577..647L. https://www.nature.com/articles/s41586-020-1938-0. Retrieved 16 October 2021.
209. ↑ Stanford, Michael G.; Bets, Ksenia V.; Luong, Duy X.; Advincula, Paul A.; Chen, Weiyin; Li, John Tianci; Wang, Zhe; McHugh, Emily A. et al. (27 October 2020). "Flash Graphene Morphologies". ACS Nano 14 (10): 13691–13699. doi:10.1021/acsnano.0c05900. ISSN 1936-0851. PMID 32909736. Bibcode: 2020ACSNa..1413691S.
210. ↑ Xu, Yang; Liu, Yunlong; Chen, Huabin; Lin, Xiao; Lin, Shisheng; Yu, Bin; Luo, Jikui (2012). "Ab initio study of energy-band modulation in graphene-based two-dimensional layered superlattices". Journal of Materials Chemistry 22 (45): 23821. doi:10.1039/C2JM35652J.
211. ↑ Liu, Zheng; Ma, Lulu; Shi, Gang; Zhou, Wu; Gong, Yongji; Lei, Sidong; Yang, Xuebei; Zhang, Jiangnan et al. (February 2013). "In-plane heterostructures of graphene and hexagonal boron nitride with controlled domain sizes". Nature Nanotechnology 8 (2): 119–124. doi:10.1038/nnano.2012.256. PMID 23353677. Bibcode: 2013NatNa...8..119L. https://www.nature.com/articles/nnano.2012.256. Retrieved 1 December 2020.
212. ↑ Félix, Isaac de Macêdo; Pereira, Luiz Felipe C. (9 February 2018). "Thermal Conductivity of Graphene-hBN Superlattice Ribbons". Scientific Reports 8 (1): 2737. doi:10.1038/s41598-018-20997-8. PMID 29426893. Bibcode: 2018NatSR...8.2737F.
213. ↑ Félix, Isaac de Macêdo; Pereira, Luiz Felipe C. (April 2020). "Suppression of coherent thermal transport in quasiperiodic graphene-hBN superlattice ribbons". Carbon 160: 335–341. doi:10.1016/j.carbon.2019.12.090. Bibcode: 2020Carbo.160..335F.
214. ↑ Félix, Isaac de Macêdo; Pereira, Luiz Felipe C. (1 May 2022). "Thermal conductivity of Thue–Morse and double-period quasiperiodic graphene-hBN superlattices". International Journal of Heat and Mass Transfer 186. doi:10.1016/j.ijheatmasstransfer.2021.122464. Bibcode: 2022IJHMT.18622464F. https://www.sciencedirect.com/science/article/abs/pii/S0017931021015623. Retrieved 6 January 2022.
215. ↑ Félix, Isaac de Macêdo (29 March 2016). Transporte térmico em nanofitas de grafeno-nitreto de boro (masterThesis). Brasil. Archived from the original on 5 March 2022. Retrieved 6 January 2022.
216. ↑ Félix, Isaac de Macêdo (4 August 2020). Condução de calor em nanofitas quase-periódicas de grafeno-hBN (doctoralThesis) (in português do Brasil). Universidade Federal do Rio Grande do Norte. Archived from the original on 2 February 2021. Retrieved 1 December 2020. 50px Text was copied from this source, which is available under a Creative Commons Attribution 4.0 International License .
217. ↑ 217.0 217.1 Tang, Libin; Ji, Rongbin; Cao, Xiangke; Lin, Jingyu; Jiang, Hongxing; Li, Xueming; Teng, Kar Seng; Luk, Chi Man et al. (2014). "Deep Ultraviolet Photoluminescence of Water-Soluble Self-Passivated Graphene Quantum Dots". ACS Nano 8 (6): 6312–6320. doi:10.1021/nn300760g. PMID 22559247.
218. ↑ 218.0 218.1 Tang, Libin; Ji, Rongbin; Li, Xueming; Bai, Gongxun; Liu, Chao Ping; Hao, Jianhua; Lin, Jingyu; Jiang, Hongxing et al. (2012). "Deep Ultraviolet to Near-Infrared Emission and Photoresponse in Layered N-Doped Graphene Quantum Dots". ACS Nano 8 (6): 5102–5110. doi:10.1021/nn501796r. PMID 24848545. https://cronfa.swan.ac.uk/Record/cronfa21239.
219. ↑ Tang, Libin; Ji, Rongbin; Li, Xueming; Teng, Kar Seng; Lau, Shu Ping (2013). "Size-Dependent Structural and Optical Characteristics of Glucose-Derived Graphene Quantum Dots". Particle & Particle Systems Characterization 30 (6): 523–531. doi:10.1002/ppsc.201200131.
220. ↑ Marcano, Daniela C.; Kosynkin, Dmitry V.; Berlin, Jacob M.; Sinitskii, Alexander; Sun, Zhengzong; Slesarev, Alexander; Alemany, Lawrence B.; Lu, Wei et al. (24 August 2010). "Improved Synthesis of Graphene Oxide". ACS Nano 4 (8): 4806–4814. doi:10.1021/nn1006368. ISSN 1936-0851. PMID 20731455. Bibcode: 2010ACSNa...4.4806M.
221. ↑ "Graphene Oxide Paper". Northwestern University. http://invo.northwestern.edu/technologies/detail/graphene-oxide-paper.
222. ↑ Eftekhari, Ali; Yazdani, Bahareh (2010). "Initiating electropolymerization on graphene sheets in graphite oxide structure". Journal of Polymer Science Part A: Polymer Chemistry 48 (10): 2204–2213. doi:10.1002/pola.23990. Bibcode: 2010JPoSA..48.2204E.
223. ↑ Nalla, Venkatram; Polavarapu, L.; Manga, K. K.; Goh, B. M.; Loh, K. P.; Xu, Q. H.; Ji, W. (2010). "Transient photoconductivity and femtosecond nonlinear optical properties of a conjugated polymer–graphene oxide composite". Nanotechnology 21 (41). doi:10.1088/0957-4484/21/41/415203. PMID 20852355. Bibcode: 2010Nanot..21O5203N. http://scholarbank.nus.edu.sg/handle/10635/53242.
224. ↑ Nair, R. R.; Wu, H. A.; Jayaram, P. N.; Grigorieva, I. V.; Geim, A. K. (2012). "Unimpeded permeation of water through helium-leak-tight graphene-based membranes". Science 335 (6067): 442–4. doi:10.1126/science.1211694. PMID 22282806. Bibcode: 2012Sci...335..442N.
225. ↑ Strilbytska, Olha; Semaniuk, Uliana; Burdyliuk, Nadia; Lushchak, Oleh (2022). "Evaluation of biological effects of graphene oxide using Drosophila". Physics and Chemistry of Solid State 2 (23): 242–248. doi:10.15330/pcss.23.2.242-248. https://journals.pnu.edu.ua/index.php/pcss/article/view/5751. Retrieved 6 February 2023.
226. ↑ Niyogi, Sandip; Bekyarova, Elena; Itkis, Mikhail E.; McWilliams, Jared L.; Hamon, Mark A.; Haddon, Robert C. (2006). "Solution Properties of Graphite and Graphene". J. Am. Chem. Soc. 128 (24): 7720–7721. doi:10.1021/ja060680r. PMID 16771469. Bibcode: 2006JAChS.128.7720N.
227. ↑ Whitby, Raymond L. D.; Korobeinyk, Alina; Glevatska, Katya V. (2011). "Morphological changes and covalent reactivity assessment of single-layer graphene oxides under carboxylic group-targeted chemistry". Carbon 49 (2): 722–725. doi:10.1016/j.carbon.2010.09.049. Bibcode: 2011Carbo..49..722W.
228. ↑ Park, Sungjin; Dikin, Dmitriy A.; Nguyen, SonBinh T.; Ruoff, Rodney S. (2009). "Graphene Oxide Sheets Chemically Cross-Linked by Polyallylamine". J. Phys. Chem. C 113 (36): 15801–15804. doi:10.1021/jp907613s.
229. ↑ Elias, D. C.; Nair, R. R.; Mohiuddin, T. M. G.; Morozov, S. V.; Blake, P.; Halsall, M. P.; Ferrari, A. C.; Boukhvalov, D. W. et al. (2009). "Control of Graphene's Properties by Reversible Hydrogenation: Evidence for Graphane". Science 323 (5914): 610–3. doi:10.1126/science.1167130. PMID 19179524. Bibcode: 2009Sci...323..610E.
230. ↑ Garcia, J. C.; de Lima, D. B.; Assali, L. V. C.; Justo, J. F. (2011). "Group IV graphene- and graphane-like nanosheets". Journal of Materials Chemistry C 115 (27): 13242–13246. doi:10.1021/jp203657w.
231. ↑ Yamada, Y.; Miyauchi, M.; Kim, J.; Hirose-Takai, K.; Sato, Y.; Suenaga, K.; Ohba, T.; Sodesawa, T. et al. (2011). "Exfoliated graphene ligands stabilizing copper cations". Carbon 49 (10): 3375–3378. doi:10.1016/j.carbon.2011.03.056. Bibcode: 2011Carbo..49.3375Y.
Yamada, Y. et al. (2011). "Exfoliated graphene ligands stabilizing copper cations". Carbon 49 (10): 3375–3378. doi:10.1016/j.carbon.2011.03.056. Bibcode: 2011Carbo..49.3375Y.
232. ↑ Yamada, Y.; Suzuki, Y.; Yasuda, H.; Uchizawa, S.; Hirose-Takai, K.; Sato, Y.; Suenaga, K.; Sato, S. (2014). "Functionalized graphene sheets coordinating metal cations". Carbon 75: 81–94. doi:10.1016/j.carbon.2014.03.036. Bibcode: 2014Carbo..75...81Y.
Yamada, Y. et al. (2014). "Functionalized graphene sheets coordinating metal cations". Carbon 75: 81–94. doi:10.1016/j.carbon.2014.03.036. Bibcode: 2014Carbo..75...81Y.
233. ↑ Li, Xinming; Zhao, Tianshuo; Wang, Kunlin; Yang, Ying; Wei, Jinquan; Kang, Feiyu; Wu, Dehai; Zhu, Hongwei (29 August 2011). "Directly Drawing Self-Assembled, Porous, and Monolithic Graphene Fiber from Chemical Vapor Deposition Grown Graphene Film and Its Electrochemical Properties". Langmuir 27 (19): 12164–71. doi:10.1021/la202380g. PMID 21875131. https://figshare.com/articles/Directly_Drawing_Self_Assembled_Porous_and_Monolithic_Graphene_Fiber_from_Chemical_Vapor_Deposition_Grown_Graphene_Film_and_Its_Electrochemical_Properties/2608015. Retrieved 1 December 2019.
234. ↑ Li, Xinming; Zhao, Tianshuo; Chen, Qiao; Li, Peixu; Wang, Kunlin; Zhong, Minlin; Wei, Jinquan; Wu, Dehai et al. (3 September 2013). "Flexible all-solid-state supercapacitors based on chemical vapor deposition derived graphene fibers". Physical Chemistry Chemical Physics 15 (41): 17752–7. doi:10.1039/C3CP52908H. PMID 24045695. Bibcode: 2013PCCP...1517752L.
235. ↑ Xin, Guoqing; Yao, Tiankai; Sun, Hongtao; Scott, Spencer Michael; Shao, Dali; Wang, Gongkai; Lian, Jie (4 September 2015). "Highly thermally conductive and mechanically strong graphene fibers". Science 349 (6252): 1083–1087. doi:10.1126/science.aaa6502. PMID 26339027. Bibcode: 2015Sci...349.1083X.
236. ↑ Xu, Zhen; Liu, Yingjun; Zhao, Xiaoli; Li, Peng; Sun, Haiyan; Xu, Yang; Ren, Xibiao; Jin, Chuanhong et al. (2016). "Ultrastiff and Strong Graphene Fibers via Full-Scale Synergetic Defect Engineering". Advanced Materials 28 (30): 6449–6456. doi:10.1002/adma.201506426. PMID 27184960. Bibcode: 2016AdM....28.6449X.
237. ↑ Bai, Yunxiang; Zhang, Rufan; Ye, Xuan; Zhu, Zhenxing; Xie, Huanhuan; Shen, Boyuan; Cai, Dali; Liu, Bofei et al. (2018). "Carbon nanotube bundles with tensile strength over 80 GPa.". Nature Nanotechnology 13 (7): 589–595. doi:10.1038/s41565-018-0141-z. PMID 29760522. Bibcode: 2018NatNa..13..589B.
238. ↑ Wang, H.; Sun, K.; Tao, F.; Stacchiola, Dario J.; Hu, Y. H. (2013). "3D Honeycomb-Like Structured Graphene and Its High Efficiency as a Counter-Electrode Catalyst for Dye-Sensitized Solar Cells". Angewandte Chemie 125 (35): 9380–9384. doi:10.1002/ange.201303497. PMID 23897636. Bibcode: 2013AngCh.125.9380W.
Wang, Hui; Sun, Kai; Tao, Franklin; Stacchiola, Dario J.; Hu, Yun Hang (2013). "3D graphene could replace expensive platinum in solar cells". Angewandte Chemie (KurzweilAI) 125 (35): 9380–9384. doi:10.1002/ange.201303497. Bibcode: 2013AngCh.125.9380W. http://www.kurzweilai.net/3d-graphene-could-replace-expensive-platinum-in-solar-cells. Retrieved 24 August 2013.
239. ↑ 239.0 239.1 239.2 Shehzad, Khurram; Xu, Yang; Gao, Chao; Xianfeng, Duan (2016). "Three-dimensional macro-structures of two-dimensional nanomaterials". Chemical Society Reviews 45 (20): 5541–5588. doi:10.1039/C6CS00218H. PMID 27459895.
240. ↑ Lalwani, Gaurav; Trinward Kwaczala, Andrea; Kanakia, Shruti; Patel, Sunny C.; Judex, Stefan; Sitharaman, Balaji (2013). "Fabrication and characterization of three-dimensional macroscopic all-carbon scaffolds.". Carbon 53: 90–100. doi:10.1016/j.carbon.2012.10.035. PMID 23436939.
241. ↑ Lalwani, Gaurav; Gopalan, Anu Gopalan; D'Agati, Michael; Srinivas Sankaran, Jeyantt; Judex, Stefan; Qin, Yi-Xian; Sitharaman, Balaji (2015). "Porous three-dimensional carbon nanotube scaffolds for tissue engineering". Journal of Biomedical Materials Research Part A 103 (10): 3212–3225. doi:10.1002/jbm.a.35449. PMID 25788440.
242. ↑ 242.0 242.1 Lapshin, Rostislav V. (January 2016). "STM observation of a box-shaped graphene nanostructure appeared after mechanical cleavage of pyrolytic graphite". Applied Surface Science 360: 451–460. doi:10.1016/j.apsusc.2015.09.222. Bibcode: 2016ApSS..360..451L.
243. ↑ Harris, P. J. F. (2012). "Hollow structures with bilayer graphene walls". Carbon 50 (9): 3195–3199. doi:10.1016/j.carbon.2011.10.050. Bibcode: 2012Carbo..50.3195H. https://zenodo.org/record/896080. Retrieved 30 August 2019.
244. ↑ Harris, P. J.; Slater, T. J.; Haigh, S. J.; Hage, F. S.; Kepaptsoglou, D. M.; Ramasse, Q. M.; Brydson, R. (2014). "Bilayer graphene formed by passage of current through graphite: evidence for a three dimensional structure". Nanotechnology 25 (46). doi:10.1088/0957-4484/25/46/465601. PMID 25354780. Bibcode: 2014Nanot..25.5601H. http://centaur.reading.ac.uk/38041/1/3D FOR NANOTECHNOLOGY SUBMITTED REVISED with figs.pdf. Retrieved 30 August 2019.
245. ↑ 245.0 245.1 245.2 245.3 "Carbon nanotubes as reinforcing bars to strengthen graphene and increase conductivity". Kurzweil Library. 9 April 2014. http://www.kurzweilai.net/carbon-nanotubes-as-reinforcing-bars-to-strengthen-graphene-and-increase-conductivity.
246. ↑ Yan, Z.; Peng, Z.; Casillas, G.; Lin, J.; Xiang, C.; Zhou, H.; Yang, Y.; Ruan, G. et al. (2014). "Rebar Graphene". ACS Nano 8 (5): 5061–8. doi:10.1021/nn501132n. PMID 24694285. Bibcode: 2014ACSNa...8.5061Y.
247. ↑ "Robust new process forms 3D shapes from flat sheets of graphene". 23 June 2015. https://grainger.illinois.edu/news/11255.
248. ↑ Jeffrey, Colin (28 June 2015). "Graphene takes on a new dimension". https://newatlas.com/3d-shapes-graphene-uiuc/38164/.
249. ↑ "How to form 3-D shapes from flat sheets of graphene". 30 June 2015. http://www.kurzweilai.net/how-to-form-3-d-shapes-from-flat-sheets-of-graphene.
250. ↑ Anthony, Sebastian (10 April 2013). "Graphene aerogel is seven times lighter than air, can balance on a blade of grass - Slideshow | ExtremeTech". http://www.extremetech.com/extreme/153063-graphene-aerogel-is-seven-times-lighter-than-air-can-balance-on-a-blade-of-grass.
251. ↑ 251.0 251.1 "Graphene nano-coils discovered to be powerful natural electromagnets". 16 October 2015. http://www.kurzweilai.net/graphene-nano-coils-discovered-to-be-powerful-natural-electromagnets.
252. ↑ Xu, Fangbo; Yu, Henry; Sadrzadeh, Arta; Yakobson, Boris I. (14 October 2015). "Riemann Surfaces of Carbon as Graphene Nanosolenoids". Nano Letters 16 (1): 34–9. doi:10.1021/acs.nanolett.5b02430. PMID 26452145. Bibcode: 2016NanoL..16...34X.
253. ↑ Stacey, Kevin (21 March 2016). "Wrinkles and crumples make graphene better | News from Brown". Brown University. https://news.brown.edu/articles/2016/03/wrinkles.
254. ↑ Chen, Po-Yen; Sodhi, Jaskiranjeet; Qiu, Yang; Valentin, Thomas M.; Steinberg, Ruben Spitz; Wang, Zhongying; Hurt, Robert H.; Wong, Ian Y. (6 May 2016). "Multiscale Graphene Topographies Programmed by Sequential Mechanical Deformation". Advanced Materials (John Wiley & Sons, Inc.) 28 (18): 3564–3571. doi:10.1002/adma.201506194. PMID 26996525. Bibcode: 2016AdM....28.3564C.
255. ↑ Backes, Claudia (2020). "Production and processing of graphene and related materials". 2D Materials 7 (2): 022001. doi:10.1088/2053-1583/ab1e0a. Bibcode: 2020TDM.....7b2001B.
256. ↑ 256.0 256.1 256.2 256.3 Whitener, Keith E.; Sheehan, Paul E. (1 June 2014). "Graphene synthesis". Diamond and Related Materials 46: 25–34. doi:10.1016/j.diamond.2014.04.006. ISSN 0925-9635. Bibcode: 2014DRM....46...25W. https://linkinghub.elsevier.com/retrieve/pii/S0925963514000983.
257. ↑ Geim, A. K.; MacDonald, A. H. (2007). "Graphene: Exploring carbon flatland". Physics Today 60 (8): 35–41. doi:10.1063/1.2774096. Bibcode: 2007PhT....60h..35G.
258. ↑ Kusmartsev, F. V.; Wu, W. M.; Pierpoint, M. P.; Yung, K. C. (2014). "Application of Graphene within Optoelectronic Devices and Transistors". arXiv:1406.0809 [cond-mat.mtrl-sci].
259. ↑ Jayasena, Buddhika; Sathyan, Subbiah (2011). "A novel mechanical cleavage method for synthesizing few-layer graphenes". Nanoscale Research Letters 6 (95): 95. doi:10.1186/1556-276X-6-95. PMID 21711598. Bibcode: 2011NRL.....6...95J.
260. ↑ Paton, Keith R.; Varrla, Eswaraiah; Backes, Claudia; Smith, Ronan J.; Khan, Umar; O'Neill, Arlene; Boland, Conor; Lotya, Mustafa et al. (2014). "Scalable production of large quantities of defect-free few-layer graphene by shear exfoliation in liquids". Nature Materials 13 (6): 624–630. doi:10.1038/nmat3944. PMID 24747780. Bibcode: 2014NatMa..13..624P. http://sro.sussex.ac.uk/id/eprint/84627/1/__smbhome.uscs.susx.ac.uk_akj23_Documents_Scalable production of large quantities.pdf.
261. ↑ ROUZAFZAY, F.; SHIDPOUR, R. (2020). "Graphene@ZnO nanocompound for short-time water treatment under sun-simulated irradiation: Effect of shear exfoliation of graphene using kitchen blender on photocatalytic degradation". Alloys and Compounds 829. doi:10.1016/J.JALLCOM.2020.154614.
262. ↑ Bor Z. Jang, "Environmentally benign process for producing graphene-protected anode particles for lithium batteries", USA patent US11038172B2, published 2020-09-10, issued 2021-06-15, assigned to Nanotek Instruments, Incand Global Graphene Group, Inc
263. ↑ Geim, A. K.; MacDonald, A. H. (2007). "Graphene: Exploring carbon flatland". Physics Today 60 (8): 35–41. doi:10.1063/1.2774096. Bibcode: 2007PhT....60h..35G.
264. ↑ Lotya, Mustafa; Hernandez, Yenny; King, Paul J.; Smith, Ronan J.; Nicolosi, Valeria; Karlsson, Lisa S.; Blighe, Fiona M.; De, Sukanta et al. (18 March 2009). "Liquid Phase Production of Graphene by Exfoliation of Graphite in Surfactant/Water Solutions". Journal of the American Chemical Society 131 (10): 3611–3620. doi:10.1021/ja807449u. PMID 19227978. Bibcode: 2009JAChS.131.3611L.
265. ↑ Backes, Claudia; Campi, Davide; Szydlowska, Beata M.; Synnatschke, Kevin; Ojala, Ezgi; Rashvand, Farnia; Harvey, Andrew; Griffin, Aideen et al. (25 June 2019). "Equipartition of Energy Defines the Size–Thickness Relationship in Liquid-Exfoliated Nanosheets". ACS Nano 13 (6): 7050–7061. doi:10.1021/acsnano.9b02234. PMID 31199123. Bibcode: 2019ACSNa..13.7050B.
266. ↑ Woltornist, S. J.; Oyer, A. J.; Carrillo, J.-M. Y.; Dobrynin, A. V; Adamson, D. H. (2013). "Conductive thin films of pristine graphene by solvent interface trapping". ACS Nano 7 (8): 7062–6. doi:10.1021/nn402371c. PMID 23879536. Bibcode: 2013ACSNa...7.7062W.
267. ↑ Coleman, Jonathan N.; Lotya, Mustafa; O'Neill, Arlene; Bergin, Shane D.; King, Paul J.; Khan, Umar; Young, Karen; Gaucher, Alexandre et al. (4 February 2011). "Two-Dimensional Nanosheets Produced by Liquid Exfoliation of Layered Materials". Science 331 (6017): 568–571. doi:10.1126/science.1194975. PMID 21292974. Bibcode: 2011Sci...331..568C.
268. ↑ Brumfiel, G. (2009). "Nanotubes cut to ribbons New techniques open up carbon tubes to create ribbons". Nature. doi:10.1038/news.2009.367.
269. ↑ Kosynkin, D. V.; Higginbotham, Amanda L.; Sinitskii, Alexander; Lomeda, Jay R.; Dimiev, Ayrat; Price, B. Katherine; Tour, James M. (2009). "Longitudinal unzipping of carbon nanotubes to form graphene nanoribbons". Nature 458 (7240): 872–6. doi:10.1038/nature07872. PMID 19370030. Bibcode: 2009Natur.458..872K.
270. ↑ Liying, Jiao; Zhang, Li; Wang, Xinran; Diankov, Georgi; Dai, Hongjie (2009). "Narrow graphene nanoribbons from carbon nanotubes". Nature 458 (7240): 877–80. doi:10.1038/nature07919. PMID 19370031. Bibcode: 2009Natur.458..877J.
271. ↑ "How to Make Graphene Using Supersonic Buckyballs | MIT Technology Review". 13 August 2015. http://www.technologyreview.com/view/539911/how-to-make-graphene-using-supersonic-buckyballs.
272. ↑ "Boehm's 1961 isolation of graphene". Graphene Times. 7 December 2009. http://graphenetimes.com/2009/12/boehms-1961-isolation-of-graphene/.
273. ↑ Geim, Andre (January 2010). "Many Pioneers in Graphene Discovery". Letters to the Editor. American Physical Society. http://www.aps.org/publications/apsnews/201001/letters.cfm.
274. ↑ Eigler, S.; Enzelberger-Heim, M.; Grimm, S.; Hofmann, P.; Kroener, W.; Geworski, A.; Dotzer, C.; Röckert, M. et al. (2013). "Wet Chemical Synthesis of Graphene". Advanced Materials 25 (26): 3583–3587. doi:10.1002/adma.201300155. PMID 23703794. Bibcode: 2013AdM....25.3583E.
275. ↑ El-Kady, M. F.; Strong, V.; Dubin, S.; Kaner, R. B. (16 March 2012). "Laser Scribing of High-Performance and Flexible Graphene-Based Electrochemical Capacitors". Science 335 (6074): 1326–1330. doi:10.1126/science.1216744. PMID 22422977. Bibcode: 2012Sci...335.1326E.
Marcus, Jennifer (15 March 2012). "Researchers develop graphene supercapacitor holding promise for portable electronics / UCLA Newsroom". Newsroom.ucla.edu. http://newsroom.ucla.edu/portal/ucla/ucla-researchers-develop-new-graphene-230478.aspx.
276. ↑ Sadri, R. (15 February 2017). "Experimental study on thermo-physical and rheological properties of stable and green reduced graphene oxide nanofluids: Hydrothermal assisted technique". Journal of Dispersion Science and Technology 38 (9): 1302–1310. doi:10.1080/01932691.2016.1234387.
277. ↑ Kamali, A. R.; Fray, D. J. (2013). "Molten salt corrosion of graphite as a possible way to make carbon nanostructures". Carbon 56: 121–131. doi:10.1016/j.carbon.2012.12.076. Bibcode: 2013Carbo..56..121K.
278. ↑ Kamali, A. R.; Fray, D. J. (2015). "Large-scale preparation of graphene by high temperature insertion of hydrogen into graphite". Nanoscale 7 (26): 11310–11320. doi:10.1039/C5NR01132A. PMID 26053881.
279. ↑ "How to tune graphene properties by introducing defects | KurzweilAI". 30 July 2015. http://www.kurzweilai.net/how-to-tune-graphene-properties-by-introducing-defects.
280. ↑ Hofmann, Mario; Chiang, Wan-Yu; Nguyễn, Tuân D; Hsieh, Ya-Ping (21 August 2015). "Controlling the properties of graphene produced by electrochemical exfoliation - IOPscience". Nanotechnology 26 (33). doi:10.1088/0957-4484/26/33/335607. PMID 26221914. Bibcode: 2015Nanot..26G5607H.
281. ↑ Tang, L.; Li, X.; Ji, R.; Teng, K. S.; Tai, G.; Ye, J.; Wei, C.; Lau, S. P. (2012). "Bottom-up synthesis of large-scale graphene oxide nanosheets". Journal of Materials Chemistry 22 (12): 5676. doi:10.1039/C2JM15944A.
282. ↑ Li, Xueming; Lau, Shu Ping; Tang, Libin; Ji, Rongbin; Yang, Peizhi (2013). "Multicolour Light emission from chlorine-doped graphene quantum dots". Journal of Materials Chemistry C 1 (44): 7308–7313. doi:10.1039/C3TC31473A.
283. ↑ Li, Lingling; Wu, Gehui; Yang, Guohai; Peng, Juan; Zhao, Jianwei; Zhu, Jun-Jie (2013). "Focusing on luminescent graphene quantum dots: current status and future perspectives". Nanoscale 5 (10): 4015–39. doi:10.1039/C3NR33849E. PMID 23579482. Bibcode: 2013Nanos...5.4015L.
284. ↑ Li, Xueming; Lau, Shu Ping; Tang, Libin; Ji, Rongbin; Yang, Peizhi (2014). "Sulphur Doping: A Facile Approach to Tune the Electronic Structure and Optical Properties of Graphene Quantum Dots". Nanoscale 6 (10): 5323–5328. doi:10.1039/C4NR00693C. PMID 24699893. Bibcode: 2014Nanos...6.5323L.
285. ↑ Choucair, M.; Thordarson, P.; Stride, J. A. (2008). "Gram-scale production of graphene based on solvothermal synthesis and sonication". Nature Nanotechnology 4 (1): 30–3. doi:10.1038/nnano.2008.365. PMID 19119279. Bibcode: 2009NatNa...4...30C.
286. ↑ Chiu, Pui Lam; Mastrogiovanni, Daniel D. T.; Wei, Dongguang; Louis, Cassandre; Jeong, Min; Yu, Guo; Saad, Peter; Flach, Carol R. et al. (4 April 2012). "Microwave- and Nitronium Ion-Enabled Rapid and Direct Production of Highly Conductive Low-Oxygen Graphene". Journal of the American Chemical Society 134 (13): 5850–5856. doi:10.1021/ja210725p. PMID 22385480. Bibcode: 2012JAChS.134.5850C.
287. ↑ Patel, Mehulkumar; Feng, Wenchun; Savaram, Keerthi; Khoshi, M. Reza; Huang, Ruiming; Sun, Jing; Rabie, Emann; Flach, Carol et al. (2015). "Microwave Enabled One-Pot, One-Step Fabrication and Nitrogen Doping of Holey Graphene Oxide for Catalytic Applications". Small 11 (27): 3358–68. doi:10.1002/smll.201403402. PMID 25683019.
288. ↑ Sutter, P. (2009). "Epitaxial graphene: How silicon leaves the scene". Nature Materials 8 (3): 171–2. doi:10.1038/nmat2392. PMID 19229263. Bibcode: 2009NatMa...8..171S. https://zenodo.org/record/1233465. Retrieved 12 April 2020.
289. ↑ Gall, N. R.; Rut'Kov, E. V.; Tontegode, A. Ya. (1997). "Two Dimensional Graphite Films on Metals and Their Intercalation". International Journal of Modern Physics B 11 (16): 1865–1911. doi:10.1142/S0217979297000976. Bibcode: 1997IJMPB..11.1865G.
290. ↑ "Samsung's graphene breakthrough could finally put the wonder material into real-world devices". ExtremeTech. 7 April 2014. http://www.extremetech.com/extreme/179874-samsungs-graphene-breakthrough-could-finally-put-the-wonder-material-into-real-world-devices.
291. ↑ Lee, J.-H.; Lee, E. K.; Joo, W.-J.; Jang, Y.; Kim, B.-S.; Lim, J. Y.; Choi, S.-H.; Ahn, S. J. et al. (2014). "Wafer-Scale Growth of Single-Crystal Monolayer Graphene on Reusable Hydrogen-Terminated Germanium". Science 344 (6181): 286–9. doi:10.1126/science.1252268. PMID 24700471. Bibcode: 2014Sci...344..286L.
292. ↑ Bansal, Tanesh; Durcan, Christopher A.; Jain, Nikhil; Jacobs-Gedrim, Robin B.; Xu, Yang; Yu, Bin (2013). "Synthesis of few-to-monolayer graphene on rutile titanium dioxide". Carbon 55: 168–175. doi:10.1016/j.carbon.2012.12.023. Bibcode: 2013Carbo..55..168B.
293. ↑ "A smarter way to grow graphene". PhysOrg.com. May 2008. http://www.physorg.com/news129980833.html.
294. ↑ Pletikosić, I.; Kralj, M.; Pervan, P.; Brako, R.; Coraux, J.; n'Diaye, A.; Busse, C.; Michely, T. (2009). "Dirac Cones and Minigaps for Graphene on Ir(111)". Physical Review Letters 102 (5). doi:10.1103/PhysRevLett.102.056808. PMID 19257540. Bibcode: 2009PhRvL.102e6808P.
295. ↑ "New process could lead to more widespread use of graphene". Gizmag.com. 28 May 2014. http://www.gizmag.com/graphene-glass-substrate-deposition/32271.
296. ↑ Liu, W.; Li, H.; Xu, C.; Khatami, Y.; Banerjee, K. (2011). "Synthesis of high-quality monolayer and bilayer graphene on copper using chemical vapor deposition". Carbon 49 (13): 4122–4130. doi:10.1016/j.carbon.2011.05.047. Bibcode: 2011Carbo..49.4122L. https://www.sciencedirect.com/science/article/abs/pii/S0008622311004106. Retrieved 8 April 2020.
297. ↑ Mattevi, Cecilia; Kim, Hokwon; Chhowalla, Manish (2011). "A review of chemical vapour deposition of graphene on copper". Journal of Materials Chemistry 21 (10): 3324–3334. doi:10.1039/C0JM02126A. Bibcode: 2011JMCh...21.3324M.
298. ↑ Martin, Steve (18 September 2014). "Purdue-based startup scales up graphene production, develops biosensors and supercapacitors". Purdue University. http://www.purdue.edu/newsroom/releases/2014/Q3/purdue-based-startup-scales-up-graphene-production,-develops-biosensors-and-supercapacitors.html.
299. ↑ "Startup scales up graphene production, develops biosensors and supercapacitors". R&D Magazine. 19 September 2014. http://www.rdmag.com/videos/2014/09/startup-scales-graphene-production-develops-biosensors-and-supercapacitors.
300. ↑ Quick, Darren (26 June 2015). "New process could usher in "graphene-driven industrial revolution"". http://www.gizmag.com/graphene-low-cost-nanocvd/38195.
301. ↑ Bointon, Thomas H.; Barnes, Matthew D.; Russo, Saverio; Craciun, Monica F. (July 2015). "High Quality Monolayer Graphene Synthesized by Resistive Heating Cold Wall Chemical Vapor Deposition". Advanced Materials 27 (28): 4200–4206. doi:10.1002/adma.201501600. PMID 26053564. Bibcode: 2015AdM....27.4200B.
302. ↑ Tao, Li; Lee, Jongho; Chou, Harry; Holt, Milo; Ruoff, Rodney S.; Akinwande, Deji (27 March 2012). "Synthesis of High Quality Monolayer Graphene at Reduced Temperature on Hydrogen-Enriched Evaporated Copper (111) Films". ACS Nano 6 (3): 2319–2325. doi:10.1021/nn205068n. PMID 22314052. Bibcode: 2012ACSNa...6.2319T.
303. ↑ 303.0 303.1 Tao, Li; Lee, Jongho; Holt, Milo; Chou, Harry; McDonnell, Stephen J.; Ferrer, Domingo A.; Babenco, Matías G.; Wallace, Robert M. et al. (15 November 2012). "Uniform Wafer-Scale Chemical Vapor Deposition of Graphene on Evaporated Cu (111) Film with Quality Comparable to Exfoliated Monolayer". The Journal of Physical Chemistry C 116 (45): 24068–24074. doi:10.1021/jp3068848.
304. ↑ 304.0 304.1 Rahimi, Somayyeh; Tao, Li; Chowdhury, Sk. Fahad; Park, Saungeun; Jouvray, Alex; Buttress, Simon; Rupesinghe, Nalin; Teo, Ken et al. (28 October 2014). "Toward 300 mm Wafer-Scalable High-Performance Polycrystalline Chemical Vapor Deposited Graphene Transistors". ACS Nano 8 (10): 10471–10479. doi:10.1021/nn5038493. PMID 25198884. Bibcode: 2014ACSNa...810471R.
305. ↑ Woltornist, Steven J.; Alamer, Fahad Alhashmi; McDannald, Austin; Jain, Menka; Sotzing, Gregory A.; Adamson, Douglas H. (1 January 2015). "Preparation of conductive graphene/graphite infused fabrics using an interface trapping method". Carbon 81: 38–42. doi:10.1016/j.carbon.2014.09.020. ISSN 0008-6223. Bibcode: 2015Carbo..81...38W. https://www.sciencedirect.com/science/article/pii/S0008622314008719.
306. ↑ Woltornist, Steven J.; Carrillo, Jan-Michael Y.; Xu, Thomas O.; Dobrynin, Andrey V.; Adamson, Douglas H. (10 February 2015). "Polymer/Pristine Graphene Based Composites: From Emulsions to Strong, Electrically Conducting Foams". Macromolecules 48 (3): 687–693. doi:10.1021/ma5024236. ISSN 0024-9297. Bibcode: 2015MaMol..48..687W. https://pubs.acs.org/doi/10.1021/ma5024236. Retrieved 13 July 2022.
307. ↑ Ward, Shawn P.; Abeykoon, Prabodha G.; McDermott, Sean T.; Adamson, Douglas H. (8 September 2020). "Effect of Aqueous Anions on Graphene Exfoliation". Langmuir 36 (35): 10421–10428. doi:10.1021/acs.langmuir.0c01569. ISSN 0743-7463. PMID 32794716. https://pubs.acs.org/doi/10.1021/acs.langmuir.0c01569. Retrieved 13 July 2022.
308. ↑ Bento, Jennifer L.; Brown, Elizabeth; Woltornist, Steven J.; Adamson, Douglas H. (January 2017). "Thermal and Electrical Properties of Nanocomposites Based on Self-Assembled Pristine Graphene". Advanced Functional Materials 27 (1). doi:10.1002/adfm.201604277. ISSN 1616-301X. Bibcode: 2017AdvFM..2704277B.
309. ↑ Woltornist, Steven J.; Varghese, Deepthi; Massucci, Daniel; Cao, Zhen; Dobrynin, Andrey V.; Adamson, Douglas H. (May 2017). "Controlled 3D Assembly of Graphene Sheets to Build Conductive, Chemically Selective and Shape-Responsive Materials". Advanced Materials 29 (18). doi:10.1002/adma.201604947. ISSN 0935-9648. PMID 28262992. Bibcode: 2017AdM....2904947W. https://onlinelibrary.wiley.com/doi/10.1002/adma.201604947. Retrieved 13 July 2022.
310. ↑ Varghese, Deepthi; Bento, Jennifer L.; Ward, Shawn P.; Adamson, Douglas H. (16 June 2020). "Self-Assembled Graphene Composites for Flow-Through Filtration". ACS Applied Materials & Interfaces 12 (26): 29692–29699. doi:10.1021/acsami.0c05831. ISSN 1944-8244. PMID 32492330. https://pubs.acs.org/doi/10.1021/acsami.0c05831. Retrieved 13 July 2022.
311. ↑ Brown, Elizabeth E. B.; Woltornist, Steven J.; Adamson, Douglas H. (15 November 2020). "PolyHIPE foams from pristine graphene: Strong, porous, and electrically conductive materials templated by a 2D surfactant". Journal of Colloid and Interface Science 580: 700–708. doi:10.1016/j.jcis.2020.07.026. ISSN 0021-9797. PMID 32712476. Bibcode: 2020JCIS..580..700B. https://www.sciencedirect.com/science/article/pii/S0021979720309048.
312. ↑ Liyanage, Chinthani D.; Varghese, Deepthi; Brown, Elizabeth E. B.; Adamson, Douglas H. (5 November 2019). "Pristine Graphene Microspheres by the Spreading and Trapping of Graphene at an Interface". Langmuir 35 (44): 14310–14315. doi:10.1021/acs.langmuir.9b02650. ISSN 0743-7463. PMID 31647673. https://pubs.acs.org/doi/10.1021/acs.langmuir.9b02650. Retrieved 13 July 2022.
313. ↑ Woltornist, Steven J.; Oyer, Andrew J.; Carrillo, Jan-Michael Y.; Dobrynin, Andrey V.; Adamson, Douglas H. (27 August 2013). "Conductive Thin Films of Pristine Graphene by Solvent Interface Trapping". ACS Nano 7 (8): 7062–7066. doi:10.1021/nn402371c. ISSN 1936-0851. PMID 23879536. Bibcode: 2013ACSNa...7.7062W. https://pubs.acs.org/doi/10.1021/nn402371c. Retrieved 13 July 2022.
314. ↑ Chen, Feiyang; Varghese, Deepthi; McDermott, Sean T.; George, Ian; Geng, Lijiang; Adamson, Douglas H. (22 October 2020). "Interface-exfoliated graphene-based conductive screen-printing inks: low-loading, low-cost, and additive-free". Scientific Reports 10 (1): 18047. doi:10.1038/s41598-020-74821-3. ISSN 2045-2322. PMID 33093555. Bibcode: 2020NatSR..1018047C.
315. ↑ Chakrabarti, A.; Lu, J.; Skrabutenas, J. C.; Xu, T.; Xiao, Z.; Maguire, J. A.; Hosmane, N. S. (2011). "Conversion of carbon dioxide to few-layer graphene". Journal of Materials Chemistry 21 (26): 9491. doi:10.1039/C1JM11227A. Bibcode: 2011JMCh...21.9491C.
316. ↑ Kim, D. Y.; Sinha-Ray, S.; Park, J. J.; Lee, J. G.; Cha, Y. H.; Bae, S. H.; Ahn, J. H.; Jung, Y. C. et al. (2014). "Self-Healing Reduced Graphene Oxide Films by Supersonic Kinetic Spraying". Advanced Functional Materials 24 (31): 4986–4995. doi:10.1002/adfm.201400732. Bibcode: 2014AdvFM..24.4986K.
317. ↑ Kim, Do-Yeon; Sinha-Ray, Suman; Park, Jung-Jae; Lee, Jong-Gun; Cha, You-Hong; Bae, Sang-Hoon; Ahn, Jong-Hyun; Jung, Yong Chae et al. (2014). "Supersonic spray creates high-quality graphene layer". Advanced Functional Materials (KurzweilAI) 24 (31): 4986–4995. doi:10.1002/adfm.201400732. Bibcode: 2014AdvFM..24.4986K. http://www.kurzweilai.net/supersonic-spray-creates-high-quality-graphene-layer. Retrieved 14 June 2014.
318. ↑ Lin, J.; Peng, Z.; Liu, Y.; Ruiz-Zepeda, F.; Ye, R.; Samuel, E. L. G.; Yacaman, M. J.; Yakobson, B. I. et al. (2014). "Laser-induced porous graphene films from commercial polymers". Nature Communications 5. doi:10.1038/ncomms6714. PMID 25493446. Bibcode: 2014NatCo...5.5714L.
319. ↑ Duy, Luong Xuan; Peng, Zhiwei; Li, Yilun; Zhang, Jibo; Ji, Yongsung; Tour, James M. (1 January 2018). "Laser-induced graphene fibers". Carbon 126: 472–479. doi:10.1016/j.carbon.2017.10.036. ISSN 0008-6223. Bibcode: 2018Carbo.126..472D. https://www.sciencedirect.com/science/article/pii/S0008622317310370.
320. ↑ Stanford, Michael G.; Bets, Ksenia V.; Luong, Duy Xuan; Advincula, Paul A.; Chen, Weiyin; Li, John Tianci; Wang, Zhe; McHugh, Emily A. et al. (27 October 2020). "Flash Graphene Morphologies". ACS Nano 14 (10): 13691–13699. doi:10.1021/acsnano.0c05900. ISSN 1936-0851. PMID 32909736. Bibcode: 2020ACSNa..1413691S. https://pubs.acs.org/doi/10.1021/acsnano.0c05900. Retrieved 16 October 2021.
321. ↑ Algozeeb, Wala A.; Savas, Paul E.; Luong, Duy Xuan; Chen, Weiyin; Kittrell, Carter; Bhat, Mahesh; Shahsavari, Rouzbeh; Tour, James M. (24 November 2020). "Flash Graphene from Plastic Waste". ACS Nano 14 (11): 15595–15604. doi:10.1021/acsnano.0c06328. ISSN 1936-0851. PMID 33119255. Bibcode: 2020ACSNa..1415595A. https://pubs.acs.org/doi/10.1021/acsnano.0c06328. Retrieved 16 October 2021.
322. ↑ Wyss, Kevin M.; Beckham, Jacob L.; Chen, Weiyin; Luong, Duy Xuan; Hundi, Prabhas; Raghuraman, Shivaranjan; Shahsavari, Rouzbeh; Tour, James M. (15 April 2021). "Converting plastic waste pyrolysis ash into flash graphene". Carbon 174: 430–438. doi:10.1016/j.carbon.2020.12.063. ISSN 0008-6223. Bibcode: 2021Carbo.174..430W.
323. ↑ Advincula, Paul A.; Luong, Duy Xuan; Chen, Weiyin; Raghuraman, Shivaranjan; Shahsavari, Rouzbeh; Tour, James M. (June 2021). "Flash graphene from rubber waste". Carbon 178: 649–656. doi:10.1016/j.carbon.2021.03.020. ISSN 0008-6223. Bibcode: 2021Carbo.178..649A.
324. ↑ "Korean researchers grow wafer-scale graphene on a silicon substrate | KurzweilAI". 21 July 2015. https://www.kurzweilai.net/korean-researchers-grow-wafer-scale-graphene-on-a-silicon-substrate.
325. ↑ Kim, Janghyuk; Lee, Geonyeop; Kim, Jihyun (20 July 2015). "Wafer-scale synthesis of multi-layer graphene by high-temperature carbon ion implantation". Applied Physics Letters 107 (3): 033104. doi:10.1063/1.4926605. Bibcode: 2015ApPhL.107c3104K.
326. ↑ Thomas, Stuart (2018). "CMOS-compatible graphene". Nature Electronics 1 (12): 612. doi:10.1038/s41928-018-0178-x.
327. ↑ Jiang, Junkai; Chu, Jae Hwan; Banerjee, Kaustav (2018). "CMOS-Compatible Doped-Multilayer-Graphene Interconnects for Next-Generation VLSI". 2018 IEEE International Electron Devices Meeting (IEDM). pp. 34.5.1–34.5.4. doi:10.1109/IEDM.2018.8614535. ISBN 978-1-7281-1987-8.
328. ↑ Template:Cite news
329. ↑ Template:Cite journal
330. ↑ Template:Cite journal
331. ↑ Template:Cite journal
332. ↑ Template:Cite journal
333. ↑ Template:Cite journal
334. ↑ Template:Cite journal
335. ↑ Template:Cite journal
336. ↑ Template:Cite journal
337. ↑ Template:Cite journal
338. ↑ Template:Cite journal
339. ↑ Template:Cite journal
340. ↑ Template:Cite journal
341. ↑ Template:Cite journal
342. ↑ Template:Cite journal
343. ↑ Template:Cite news
344. ↑ Template:Cite web
345. ↑ Template:Cite web
346. ↑ Template:Cite journal
347. ↑ Template:Cite journal
348. ↑ Template:Cite web
349. ↑ Template:Cite web
350. ↑ Template:Cite journal
351. ↑ Template:Cite web
352. ↑ Template:Cite web
353. ↑ Template:Cite journal
354. ↑ Template:Cite journal
355. ↑ Template:Cite journal
356. ↑ Template:Cite journal
357. ↑ Template:Cite journal
358. ↑ Template:Cite book
359. ↑ Template:Cite journal
360. ↑ Template:Cite journal
361. ↑ Template:Cite journal
362. ↑ Template:Cite journal
363. ↑ Template:Cite journal
364. ↑ Template:Cite journal
365. ↑ Template:Cite web
366. ↑ Template:Cite journal

## External links

* Manchester's Revolutionary 2D Material at The University of Manchester
* Graphene at The Periodic Table of Videos (University of Nottingham)
* Graphene: Patent surge reveals global race
* 'Engineering Controls for Nano-scale Graphene Platelets During Manufacturing and Handling Processes' (PDF)
* Band structure of graphene (PDF).

Template:Allotropes of carbon Template:Emerging technologies Template:Molecules detected in outer space

Template:Sourceattribution

Retrieved from "https://handwiki.org/wiki/index.php?title=Physics:Graphene&oldid=4358638"